
#=======================================================================
data_global
#=======================================================================

_audit_creation_method                   'Jana2006 Version : 13/05/2019'


# 1. PROCESSING SUMMARY (IUCr Office Use Only)

_journal_date_recd_electronic            ?
_journal_date_to_coeditor                ?
_journal_date_from_coeditor              ?
_journal_date_accepted                   ?
_journal_date_printers_first             ?
_journal_date_printers_final             ?
_journal_date_proofs_out                 ?
_journal_date_proofs_in                  ?
_journal_coeditor_name                   ?
_journal_coeditor_code                   ?
_journal_coeditor_notes
; ?
;
_journal_techeditor_code                 ?
_journal_paper_category                  ?
_journal_techeditor_notes
; ?
;
_journal_coden_ASTM                      ?
_journal_name_full                       'Dalton Trans.'
_journal_year                            ?
_journal_volume                          ?
_journal_issue                           ?
_journal_page_first                      ?
_journal_page_last                       ?
_journal_suppl_publ_number               ?
_journal_suppl_publ_pages                ?

#=======================================================================

# 2. SUBMISSION DETAILS

_publ_contact_author_name                'Dr. Oliver Janka'
_publ_contact_author_address     
;Institut für Anorganische und Analytische Chemie
Corrensstrasse 30
48149 Münster
;
_publ_contact_author_email       ocjanka@uni-muenster.de
_publ_contact_author_phone       '0049 251 83-36047'
_publ_contact_author_fax         '0049 251 83-36002'

_publ_requested_journal                  'Dalton Transactions'
_publ_requested_category                 ?

_publ_contact_letter
; ?
;

#=======================================================================

# 3. TITLE AND AUTHOR LIST

_publ_section_title
; ?
;
_publ_section_title_footnote
; ?
;
loop_
 _publ_author_name
 _publ_author_address
      'Frank Stegemann, MSc.'
;      Institut für Anorganische und Analytische Chemie
       Westfälische Wilhelms-Universität Münster
       Corrensstrasse 28/30
       48149 Münster
       Bundesrepublik Deutschland
;
      'Rachid St. Touzani'
;      Institut für Werkstoff- und Fügetechnik (IWF)
       Otto-von-Guericke-Universität Magdeburg
       Grosse Steinernetischstrasse 6
       39104 Magdeburg
       Bundesrepublik Deutschland
;
      'Priv.-Doz. Dr. Oliver Janka'
;      Institut für Anorganische und Analytische Chemie
       Westfälische Wilhelms-Universität Münster
       Corrensstrasse 28/30
       48149 Münster
       Bundesrepublik Deutschland
;
#=======================================================================

# 4. TEXT

_publ_section_synopsis
; ?
;
_publ_section_abstract
; ?
;
_publ_section_comment
; ?
;
_publ_section_introduction
; ?
;
_publ_section_experimental
; ?
;
_publ_section_exptl_prep
; ?
;
_publ_section_exptl_refinement
; ?
;
_publ_section_exptl_solution
; ?
;
_publ_section_discussion
; ?
;
_publ_section_acknowledgements
; ?
;
_publ_section_references
;
Petricek, V., Dusek, M. & Palatinus L. (2014). Z. Kristallogr. 229(5), 345-352.

Palatinus L. & Chapuis G. (2007). J. Appl. Cryst. 40, 786-790.

# enable this reference if Diamond ver. 2 was used for visualization
#Brandenburg, K. (1999). DIAMOND. Version. 2.1c.
#Crystal Impact GbR, Bonn, Germany.

# enable this reference if Diamond ver. 3 was used for visualization
#Brandenburg, K. & Putz, H. (2005). DIAMOND Version 3.
#Crystal Impact GbR, Postfach 1251, D-53002 Bonn, Germany.

# enable this reference if SIR97 was used for solving of the structure
#Altomare, A., Burla, M. C., Camalli, M., Cascarano, G., Giacovazzo, C.,
#Guagliardi, A., Moliterni, A. G. G., Polidori, G., Spagna, R. (1997).
#SIR97. A Package for Crystal Structure Solution by Direct Methods
#and Refinement, Bari, Rome, Italy.

# use this reference if SIR2002 was used for solving of the structure
#Burla, M.C., Camalli, M., Carrozzini, B., Cascarano, G., Giacovazzo, C.,
#Polidori, G., Spagna, R.
#SIR2002: the program, J. Appl. Cryst, (2003). 36, 1103


# use this reference if SIR2011 was used for solving of the structure
#Burla, M.C., Caliandro, R., Camalli, M., Carrozzini, B., Cascarano,
#G.L., Giacovazzo, C., Mallamo. M., Mazzone, A., Polidori, G., Spagna, R.
#SIR2011: a new package for crystal structure determination and refinement,
#J.Appl.Cryst. (2012) 45, 357-361

# enable this reference if bond valences were calculated
#Brown, I. D. (1996). J. Appl. Cryst. 29, 479-480.

# enable this reference if Xshape wase used for crystal shape refinement
#Stoe & Cie (1998). X-SHAPE. Stoe & Cie, Darmstadt, Germany.


# enable this reference if Flack coefficient was refined
#Flack, H. D. (1983). Acta Cryst. A39, 876-881.
;
_publ_section_figure_captions
; ?
;
_publ_section_table_legends
; ?
;

#=======================================================================
data_I
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic
; ?
;
_chemical_name_common                    ?
_chemical_formula_moiety                 ?
_chemical_formula_structural             ?
_chemical_formula_analytical             ?
_chemical_formula_iupac                  ?
_chemical_formula_sum                    'Al53 Ba6 Pt21.96'
_chemical_formula_weight                 6538.8
_chemical_melting_point                  ?
_chemical_compound_source                ?
_chemical_absolute_configuration         .

#=======================================================================

# 6. CRYSTAL DATA

_symmetry_cell_setting                   hexagonal
_symmetry_space_group_name_H-M           'P 63/m c m'
_symmetry_space_group_name_Hall          '-P 6c;-2'
_symmetry_Int_Tables_number              193

loop_
 _space_group_symop_id
 _space_group_symop_operation_xyz
 1   x,y,z
 2   -y,x-y,z
 3   -x+y,-x,z
 4   -x,-y,z+1/2
 5   y,-x+y,z+1/2
 6   x-y,x,z+1/2
 7   y,x,-z+1/2
 8   x-y,-y,-z+1/2
 9   -x,-x+y,-z+1/2
 10  -y,-x,-z
 11  -x+y,y,-z
 12  x,x-y,-z
 13  -x,-y,-z
 14  y,-x+y,-z
 15  x-y,x,-z
 16  x,y,-z+1/2
 17  -y,x-y,-z+1/2
 18  -x+y,-x,-z+1/2
 19  -y,-x,z+1/2
 20  -x+y,y,z+1/2
 21  x,x-y,z+1/2
 22  y,x,z
 23  x-y,-y,z
 24  -x,-x+y,z

_cell_length_a                           14.2490(2)
_cell_length_b                           14.2490(2)
_cell_length_c                           16.1127(3)
_cell_angle_alpha                        90
_cell_angle_beta                         90
_cell_angle_gamma                        120
_cell_volume                             2833.1

loop_
 _twin_individual_id
 _twin_individual_mass_fraction_refined
 _twin_individual_twin_matrix_11
 _twin_individual_twin_matrix_12
 _twin_individual_twin_matrix_13
 _twin_individual_twin_matrix_21
 _twin_individual_twin_matrix_22
 _twin_individual_twin_matrix_23
 _twin_individual_twin_matrix_31
 _twin_individual_twin_matrix_32
 _twin_individual_twin_matrix_33
 ? ? ? ? ? ? ? ? ? ? ?

_cell_formula_units_Z                    2

_cell_measurement_reflns_used            80707
_cell_measurement_theta_min              2.52
_cell_measurement_theta_max              31.4
_cell_measurement_temperature            90
_cell_special_details
; ?
;

_exptl_crystal_density_diffrn            7.67
_exptl_crystal_density_meas              ?
_exptl_crystal_density_method            ?
_exptl_crystal_F_000                     5473

_exptl_absorpt_coefficient_mu            58.9
_exptl_crystal_description               block
_exptl_crystal_size_max                  0.080
_exptl_crystal_size_mid                  0.055
_exptl_crystal_size_min                  0.040
_exptl_crystal_size_rad                  ?
_exptl_crystal_colour                    silver
_exptl_absorpt_correction_type           numerical
_exptl_absorpt_process_details           ?
_exptl_absorpt_correction_T_min          0.040
_exptl_absorpt_correction_T_max          0.170
loop_
 _exptl_crystal_face_index_h
 _exptl_crystal_face_index_k
 _exptl_crystal_face_index_l
 _exptl_crystal_face_perp_dist
 ? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details                   ?

_diffrn_ambient_temperature              90
_diffrn_source                           ?
_diffrn_source_power                     ?
_diffrn_source_voltage                   ?
_diffrn_source_current                   ?
_diffrn_radiation_type                   'Mo K\a'
_diffrn_radiation_source                 'X-ray tube'
_diffrn_radiation_wavelength             0.71073
_diffrn_radiation_monochromator          graphite
_diffrn_measurement_device               'four-circle diffractometer'
_diffrn_measurement_device_type          'Stoe StadiVari'
_diffrn_detector                         ?
_diffrn_detector_area_resol_mean         ?
_diffrn_measurement_method               '??integration method??'
_diffrn_measurement_specimen_support     ?

_diffrn_reflns_number                    91439
_diffrn_reflns_theta_min                 2.53
_diffrn_reflns_theta_max                 31.08
_diffrn_reflns_theta_full                31.08
_diffrn_measured_fraction_theta_max      1
_diffrn_measured_fraction_theta_full     1
_diffrn_reflns_av_R_equivalents          0.0490
_diffrn_reflns_av_unetI/netI             0.0071
_diffrn_reflns_limit_h_min               -20
_diffrn_reflns_limit_h_max               20
_diffrn_reflns_limit_k_min               -20
_diffrn_reflns_limit_k_max               20
_diffrn_reflns_limit_l_min               -23
_diffrn_reflns_limit_l_max               23
_diffrn_reflns_reduction_process         ?

_diffrn_standards_number                 ?
_diffrn_standards_interval_count         ?
_diffrn_standards_interval_time          ?
_diffrn_standards_decay_%                ?
loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
  ? ? ?

_diffrn_radiation_probe                  X-ray

#=======================================================================

# 8. REFINEMENT DATA

_refine_special_details
; ?
;

_reflns_number_total                     1665
_reflns_number_gt                        1260
_reflns_threshold_expression             'I>3σ(I)'

_refine_ls_structure_factor_coef         Fsqd
_refine_ls_R_factor_gt                   0.0221
_refine_ls_wR_factor_gt                  0.0573
_refine_ls_R_factor_all                  0.0328
_refine_ls_wR_factor_ref                 0.0594
_refine_ls_goodness_of_fit_ref           1.73
_refine_ls_goodness_of_fit_gt            1.93
_refine_ls_restrained_S_gt               ?
_refine_ls_restrained_S_all              ?
_refine_ls_number_reflns                 1665
_refine_ls_number_parameters             86
_refine_ls_number_restraints             0
_refine_ls_number_constraints            0
_refine_ls_weighting_scheme              sigma
_refine_ls_weighting_details             'w=1/(σ²(I)+0.0004I²)'
_refine_ls_hydrogen_treatment            ?
_refine_ls_shift/su_max                  0.0005
_refine_ls_shift/su_mean                 0.0001
_refine_diff_density_max                 1.92
_refine_diff_density_min                 -1.77
_refine_ls_extinction_method
 'B-C type 1 Lorentzian isotropic (Becker & Coppens, 1974)'
_refine_ls_extinction_coef               120(20)
_refine_ls_extinction_expression         ?
_refine_ls_abs_structure_details         ?
_refine_ls_abs_structure_Flack           ?
_refine_ls_abs_structure_Rogers          ?

loop_
 _atom_type_symbol
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 Al   0.0645  0.0514
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Ba  -0.3244  2.2819
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
 Pt  -1.7033  8.3905
 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection               ?
_computing_cell_refinement               ?
_computing_data_reduction                ?
_computing_structure_solution            ?
_computing_structure_refinement          ?
_computing_molecular_graphics            ?
_computing_publication_material          ?

loop_
 _restr_distance_atom_site_label_1
 _restr_distance_site_symmetry_1
 _restr_distance_atom_site_label_2
 _restr_distance_site_symmetry_2
 _restr_distance_target
 _restr_distance_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_angle_atom_site_label_1
 _restr_angle_site_symmetry_1
 _restr_angle_atom_site_label_2
 _restr_angle_site_symmetry_2
 _restr_angle_atom_site_label_3
 _restr_angle_site_symmetry_3
 _restr_angle_target
 _restr_angle_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_torsion_atom_site_label_1
 _restr_torsion_site_symmetry_1
 _restr_torsion_atom_site_label_2
 _restr_torsion_site_symmetry_2
 _restr_torsion_atom_site_label_3
 _restr_torsion_site_symmetry_3
 _restr_torsion_atom_site_label_4
 _restr_torsion_site_symmetry_4
 _restr_torsion_angle_target
 _restr_torsion_weight_param
 ? ? ? ? ? ? ? ? ? ?

loop_
 _restr_equal_distance_atom_site_label_1
 _restr_equal_distance_site_symmetry_1
 _restr_equal_distance_atom_site_label_2
 _restr_equal_distance_site_symmetry_2
 _restr_equal_distance_class_class_id
 _restr_equal_distance_class_target_weight_param
 ? ? ? ? ? ?

loop_
 _restr_equal_angle_atom_site_label_1
 _restr_equal_angle_site_symmetry_1
 _restr_equal_angle_atom_site_label_2
 _restr_equal_angle_site_symmetry_2
 _restr_equal_angle_atom_site_label_3
 _restr_equal_angle_site_symmetry_3
 _restr_equal_angle_class_class_id
 _restr_equal_angle_class_target_weight_param
 ? ? ? ? ? ? ? ?

loop_
 _restr_equal_torsion_atom_site_label_1
 _restr_equal_torsion_site_symmetry_1
 _restr_equal_torsion_atom_site_label_2
 _restr_equal_torsion_site_symmetry_2
 _restr_equal_torsion_atom_site_label_3
 _restr_equal_torsion_site_symmetry_3
 _restr_equal_torsion_atom_site_label_4
 _restr_equal_torsion_site_symmetry_4
 _restr_equal_torsion_class_class_id
 _restr_equal_torsion_class_target_weight_param
 ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 9. ATOMIC COORDINATES AND DISPLACEMENT PARAMETERS

loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_adp_type
 _atom_site_U_iso_or_equiv
 _atom_site_site_symmetry_multiplicity
 _atom_site_occupancy
 _atom_site_calc_flag
 _atom_site_refinement_flags
 _atom_site_disorder_assembly
 _atom_site_disorder_group
  Ba Ba 0.25013(4) 0 0.06624(3) Uani 0.01420(14) 12 1 d . . .
  Pt1 Pt 0.50225(2) 0 0.14019(2) Uani 0.01311(10) 12 1 d . . .
  Pt2 Pt 0.16813(3) 0.33805(2) 0.25 Uani 0.01321(12) 12 1 d . . .
  Pt3 Pt 0.243522(13) 0.48704(3) 0 Uani 0.01301(9) 12 1 d . . .
  Pt4 Pt 0 0 0.14784(10) Uani 0.0161(7) 4 0.982(6) d . . .
  Pt5 Pt 0.333333 0.666667 0.25 Uani 0.01331(13) 4 1 d . . .
  Al1 Al 0.17647(17) 0.49201(16) 0.15554(14) Uani 0.0148(7) 24 1 d . . .
  Al2 Al 0.28626(16) 0.39282(16) 0.11062(12) Uani 0.0142(7) 24 1 d . . .
  Al3 Al 0.8140(2) 0 0.16345(19) Uani 0.0154(8) 12 1 d . . .
  Al4 Al 0.3676(3) 0.5028(2) 0.25 Uani 0.0149(10) 12 1 d . . .
  Al5 Al 0.55483(10) 0.1097(2) 0 Uani 0.0145(7) 12 1 d . . .
  Al6 Al 0.333333 0.666667 0.0834(2) Uani 0.0141(7) 8 1 d . . .
  Al7 Al 0.1444(3) 0 0.25 Uani 0.0148(12) 6 1 d . . .
  Al8 Al 0.3620(3) 0 0.25 Uani 0.0141(11) 6 1 d . . .
  Al9 Al 0 0 0 Uani 0.0188(16) 2 1 d . . .


loop_
 _jana_atom_site_ADP_C_label
 _jana_atom_site_ADP_C_type_symbol
 _jana_atom_site_ADP_C_111
 _jana_atom_site_ADP_C_112
 _jana_atom_site_ADP_C_113
 _jana_atom_site_ADP_C_122
 _jana_atom_site_ADP_C_123
 _jana_atom_site_ADP_C_133
 _jana_atom_site_ADP_C_222
 _jana_atom_site_ADP_C_223
 _jana_atom_site_ADP_C_233
 _jana_atom_site_ADP_C_333
 Pt4 Pt 0 0 0 0 0 0 0 0 0 0

loop_
 _jana_atom_site_ADP_D_label
 _jana_atom_site_ADP_D_type_symbol
 _jana_atom_site_ADP_D_1111
 _jana_atom_site_ADP_D_1112
 _jana_atom_site_ADP_D_1113
 _jana_atom_site_ADP_D_1122
 _jana_atom_site_ADP_D_1123
 _jana_atom_site_ADP_D_1133
 _jana_atom_site_ADP_D_1222
 _jana_atom_site_ADP_D_1223
 _jana_atom_site_ADP_D_1233
 _jana_atom_site_ADP_D_1333
 _jana_atom_site_ADP_D_2222
 _jana_atom_site_ADP_D_2223
 _jana_atom_site_ADP_D_2233
 _jana_atom_site_ADP_D_2333
 _jana_atom_site_ADP_D_3333
 Pt4 Pt 0 0 0 0 0 0 0 0 0 0 0 0 0 0 0

loop_
 _jana_atom_site_ADP_E_label
 _jana_atom_site_ADP_E_type_symbol
 _jana_atom_site_ADP_E_11111
 _jana_atom_site_ADP_E_11112
 _jana_atom_site_ADP_E_11113
 _jana_atom_site_ADP_E_11122
 _jana_atom_site_ADP_E_11123
 _jana_atom_site_ADP_E_11133
 _jana_atom_site_ADP_E_11222
 _jana_atom_site_ADP_E_11223
 _jana_atom_site_ADP_E_11233
 _jana_atom_site_ADP_E_11333
 _jana_atom_site_ADP_E_12222
 _jana_atom_site_ADP_E_12223
 _jana_atom_site_ADP_E_12233
 _jana_atom_site_ADP_E_12333
 _jana_atom_site_ADP_E_13333
 _jana_atom_site_ADP_E_22222
 _jana_atom_site_ADP_E_22223
 _jana_atom_site_ADP_E_22233
 _jana_atom_site_ADP_E_22333
 _jana_atom_site_ADP_E_23333
 _jana_atom_site_ADP_E_33333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?

loop_
 _jana_atom_site_ADP_F_label
 _jana_atom_site_ADP_F_type_symbol
 _jana_atom_site_ADP_F_111111
 _jana_atom_site_ADP_F_111112
 _jana_atom_site_ADP_F_111113
 _jana_atom_site_ADP_F_111122
 _jana_atom_site_ADP_F_111123
 _jana_atom_site_ADP_F_111133
 _jana_atom_site_ADP_F_111222
 _jana_atom_site_ADP_F_111223
 _jana_atom_site_ADP_F_111233
 _jana_atom_site_ADP_F_111333
 _jana_atom_site_ADP_F_112222
 _jana_atom_site_ADP_F_112223
 _jana_atom_site_ADP_F_112233
 _jana_atom_site_ADP_F_112333
 _jana_atom_site_ADP_F_113333
 _jana_atom_site_ADP_F_122222
 _jana_atom_site_ADP_F_122223
 _jana_atom_site_ADP_F_122233
 _jana_atom_site_ADP_F_122333
 _jana_atom_site_ADP_F_123333
 _jana_atom_site_ADP_F_133333
 _jana_atom_site_ADP_F_222222
 _jana_atom_site_ADP_F_222223
 _jana_atom_site_ADP_F_222233
 _jana_atom_site_ADP_F_222333
 _jana_atom_site_ADP_F_223333
 _jana_atom_site_ADP_F_233333
 _jana_atom_site_ADP_F_333333
 ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 10. MOLECULAR GEOMETRY


loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_site_symmetry_1
 _geom_bond_site_symmetry_2
 _geom_bond_distance
 _geom_bond_publ_flag
  Ba Pt1 . . 3.7849(9) ?
  Ba Pt2 . 3_555 3.6159(6) ?
  Ba Pt2 . 7_555 3.6159(6) ?
  Ba Pt3 . 3_555 3.5864(8) ?
  Ba Pt3 . 14_555 3.5864(10) ?
  Ba Pt4 . . 3.7989(10) ?
  Ba Al1 . 3_555 3.407(3) ?
  Ba Al1 . 22_555 3.407(2) ?
  Ba Al2 . 3_555 3.604(2) ?
  Ba Al2 . 12_555 3.387(3) ?
  Ba Al2 . 14_555 3.387(2) ?
  Ba Al2 . 22_555 3.604(2) ?
  Ba Al3 . 2_545 3.5686(18) ?
  Ba Al3 . 3_665 3.569(3) ?
  Ba Al3 . 11_655 3.812(3) ?
  Ba Al5 . . 3.9556(18) ?
  Ba Al5 . 13_655 3.956(3) ?
  Ba Al7 . . 3.3222(18) ?
  Ba Al8 . . 3.362(2) ?
  Ba Al9 . . 3.7204(9) ?
  Pt1 Pt1 . 8_555 3.5388(5) ?
  Pt1 Al1 . 3_555 2.602(2) ?
  Pt1 Al1 . 22_555 2.602(3) ?
  Pt1 Al2 . 2_655 2.653(3) ?
  Pt1 Al2 . 24_655 2.653(2) ?
  Pt1 Al4 . 2_655 2.590(4) ?
  Pt1 Al4 . 9_655 2.590(2) ?
  Pt1 Al5 . . 2.6333(14) ?
  Pt1 Al5 . 13_655 2.6333(14) ?
  Pt1 Al8 . . 2.670(3) ?
  Pt2 Al1 . . 2.624(2) ?
  Pt2 Al1 . 16_555 2.624(2) ?
  Pt2 Al2 . . 2.678(2) ?
  Pt2 Al2 . 16_555 2.678(2) ?
  Pt2 Al3 . 3_665 2.693(3) ?
  Pt2 Al3 . 9_665 2.693(3) ?
  Pt2 Al4 . . 2.630(3) ?
  Pt2 Al7 . 2_555 2.597(2) ?
  Pt2 Al8 . 2_555 2.583(2) ?
  Pt3 Pt3 . 2_665 3.8391(12) ?
  Pt3 Pt3 . 3_565 3.8391(9) ?
  Pt3 Al1 . . 2.696(2) ?
  Pt3 Al1 . 11_555 2.696(2) ?
  Pt3 Al2 . . 2.484(2) ?
  Pt3 Al2 . 11_555 2.484(2) ?
  Pt3 Al5 . 14_565 2.533(4) ?
  Pt3 Al5 . 15_555 2.533(3) ?
  Pt3 Al6 . . 2.5919(18) ?
  Pt3 Al6 . 10_665 2.5919(18) ?
  Pt4 Pt4 . 7_555 3.292(2) ?
  Pt4 Al3 . 1_455 2.663(3) ?
  Pt4 Al3 . 2_545 2.663(3) ?
  Pt4 Al3 . 3_665 2.663(2) ?
  Pt4 Al7 . . 2.635(3) ?
  Pt4 Al7 . 2_555 2.635(3) ?
  Pt4 Al7 . 3_555 2.635(2) ?
  Pt4 Al9 . . 2.3821(17) ?
  Pt5 Al1 . . 2.8184(19) ?
  Pt5 Al1 . 2_665 2.818(3) ?
  Pt5 Al1 . 3_565 2.818(3) ?
  Pt5 Al1 . 16_555 2.8184(19) ?
  Pt5 Al1 . 17_665 2.818(3) ?
  Pt5 Al1 . 18_565 2.818(3) ?
  Pt5 Al4 . . 2.613(4) ?
  Pt5 Al4 . 2_665 2.613(3) ?
  Pt5 Al4 . 3_565 2.613(5) ?
  Pt5 Al6 . . 2.685(3) ?
  Pt5 Al6 . 16_555 2.685(3) ?
  Al1 Al1 . 16_555 3.044(3) ?
  Al1 Al2 . . 2.679(4) ?
  Al1 Al2 . 3_565 3.827(4) ?
  Al1 Al4 . . 3.056(4) ?
  Al1 Al4 . 3_565 2.800(5) ?
  Al1 Al5 . 14_565 2.973(3) ?
  Al1 Al6 . . 2.642(2) ?
  Al1 Al8 . 2_555 2.723(2) ?
  Al2 Al2 . 22_555 2.630(4) ?
  Al2 Al3 . 3_665 2.690(3) ?
  Al2 Al4 . . 2.651(2) ?
  Al2 Al4 . 7_555 3.975(4) ?
  Al2 Al5 . 3_665 3.940(4) ?
  Al2 Al5 . 15_555 2.899(2) ?
  Al2 Al6 . . 3.640(3) ?
  Al3 Al3 . 8_555 2.789(4) ?
  Al3 Al7 . 2_655 2.784(3) ?
  Al3 Al7 . 3_655 2.784(5) ?
  Al3 Al9 . 1_655 3.737(3) ?
  Al4 Al4 . 7_555 3.337(6) ?
  Al4 Al6 . . 3.747(4) ?
  Al4 Al6 . 16_555 3.747(4) ?
  Al4 Al8 . 3_665 3.337(5) ?
  Al5 Al5 . 13_655 2.706(4) ?
  Al5 Al6 . 13_665 3.070(3) ?
  Al5 Al6 . 22_555 3.070(3) ?
  Al6 Al6 . 10_665 2.687(5) ?
  Al7 Al7 . 2_555 3.563(5) ?
  Al7 Al7 . 3_555 3.563(5) ?
  Al7 Al8 . . 3.100(6) ?

loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_2
 _geom_angle_site_symmetry_3
 _geom_angle
 _geom_angle_publ_flag
  Pt1 Ba Pt2 . . 3_555 74.206(14) ?
  Pt1 Ba Pt2 . . 7_555 74.206(12) ?
  Pt1 Ba Pt3 . . 3_555 70.088(11) ?
  Pt1 Ba Pt3 . . 14_555 70.087(13) ?
  Pt1 Ba Pt4 . . . 141.40(3) ?
  Pt1 Ba Al1 . . 3_555 42.02(4) ?
  Pt1 Ba Al1 . . 22_555 42.02(5) ?
  Pt1 Ba Al2 . . 3_555 86.51(5) ?
  Pt1 Ba Al2 . . 12_555 84.71(5) ?
  Pt1 Ba Al2 . . 14_555 84.71(5) ?
  Pt1 Ba Al2 . . 22_555 86.51(4) ?
  Pt1 Ba Al3 . . 2_545 117.21(4) ?
  Pt1 Ba Al3 . . 3_665 117.21(5) ?
  Pt1 Ba Al3 . . 11_655 122.21(5) ?
  Pt1 Ba Al5 . . . 39.70(3) ?
  Pt1 Ba Al5 . . 13_655 39.700(13) ?
  Pt1 Ba Al7 . . . 98.62(6) ?
  Pt1 Ba Al8 . . . 43.36(6) ?
  Pt1 Ba Al9 . . . 178.323(17) ?
  Pt2 Ba Pt2 3_555 . 7_555 70.031(13) ?
  Pt2 Ba Pt3 3_555 . 3_555 75.875(10) ?
  Pt2 Ba Pt3 3_555 . 14_555 135.852(16) ?
  Pt2 Ba Pt4 3_555 . . 74.38(2) ?
  Pt2 Ba Al1 3_555 . 3_555 43.75(5) ?
  Pt2 Ba Al1 3_555 . 22_555 90.64(4) ?
  Pt2 Ba Al2 3_555 . 3_555 43.54(3) ?
  Pt2 Ba Al2 3_555 . 12_555 117.42(5) ?
  Pt2 Ba Al2 3_555 . 14_555 154.95(6) ?
  Pt2 Ba Al2 3_555 . 22_555 113.57(3) ?
  Pt2 Ba Al3 3_555 . 2_545 44.03(4) ?
  Pt2 Ba Al3 3_555 . 3_665 91.10(5) ?
  Pt2 Ba Al3 3_555 . 11_655 143.000(16) ?
  Pt2 Ba Al5 3_555 . . 113.80(3) ?
  Pt2 Ba Al5 3_555 . 13_655 90.63(3) ?
  Pt2 Ba Al7 3_555 . . 43.70(3) ?
  Pt2 Ba Al8 3_555 . . 43.26(3) ?
  Pt2 Ba Al9 3_555 . . 104.445(15) ?
  Pt2 Ba Pt3 7_555 . 3_555 135.852(16) ?
  Pt2 Ba Pt3 7_555 . 14_555 75.875(9) ?
  Pt2 Ba Pt4 7_555 . . 74.38(2) ?
  Pt2 Ba Al1 7_555 . 3_555 90.64(4) ?
  Pt2 Ba Al1 7_555 . 22_555 43.75(4) ?
  Pt2 Ba Al2 7_555 . 3_555 113.57(3) ?
  Pt2 Ba Al2 7_555 . 12_555 154.95(4) ?
  Pt2 Ba Al2 7_555 . 14_555 117.42(4) ?
  Pt2 Ba Al2 7_555 . 22_555 43.54(3) ?
  Pt2 Ba Al3 7_555 . 2_545 91.10(5) ?
  Pt2 Ba Al3 7_555 . 3_665 44.03(5) ?
  Pt2 Ba Al3 7_555 . 11_655 143.000(16) ?
  Pt2 Ba Al5 7_555 . . 90.63(2) ?
  Pt2 Ba Al5 7_555 . 13_655 113.80(2) ?
  Pt2 Ba Al7 7_555 . . 43.70(3) ?
  Pt2 Ba Al8 7_555 . . 43.26(3) ?
  Pt2 Ba Al9 7_555 . . 104.445(14) ?
  Pt3 Ba Pt3 3_555 . 14_555 113.841(18) ?
  Pt3 Ba Pt4 3_555 . . 122.158(12) ?
  Pt3 Ba Al1 3_555 . 3_555 45.25(4) ?
  Pt3 Ba Al1 3_555 . 22_555 111.55(5) ?
  Pt3 Ba Al2 3_555 . 3_555 40.41(5) ?
  Pt3 Ba Al2 3_555 . 12_555 41.60(5) ?
  Pt3 Ba Al2 3_555 . 14_555 84.42(6) ?
  Pt3 Ba Al2 3_555 . 22_555 151.77(4) ?
  Pt3 Ba Al3 3_555 . 2_545 83.03(5) ?
  Pt3 Ba Al3 3_555 . 3_665 163.07(4) ?
  Pt3 Ba Al3 3_555 . 11_655 79.67(2) ?
  Pt3 Ba Al5 3_555 . . 78.14(4) ?
  Pt3 Ba Al5 3_555 . 13_655 38.85(3) ?
  Pt3 Ba Al7 3_555 . . 118.21(2) ?
  Pt3 Ba Al8 3_555 . . 92.59(3) ?
  Pt3 Ba Al9 3_555 . . 110.666(12) ?
  Pt3 Ba Pt4 14_555 . . 122.158(13) ?
  Pt3 Ba Al1 14_555 . 3_555 111.55(5) ?
  Pt3 Ba Al1 14_555 . 22_555 45.25(4) ?
  Pt3 Ba Al2 14_555 . 3_555 151.77(6) ?
  Pt3 Ba Al2 14_555 . 12_555 84.42(4) ?
  Pt3 Ba Al2 14_555 . 14_555 41.60(4) ?
  Pt3 Ba Al2 14_555 . 22_555 40.41(4) ?
  Pt3 Ba Al3 14_555 . 2_545 163.07(5) ?
  Pt3 Ba Al3 14_555 . 3_665 83.03(4) ?
  Pt3 Ba Al3 14_555 . 11_655 79.67(2) ?
  Pt3 Ba Al5 14_555 . . 38.85(4) ?
  Pt3 Ba Al5 14_555 . 13_655 78.14(3) ?
  Pt3 Ba Al7 14_555 . . 118.21(2) ?
  Pt3 Ba Al8 14_555 . . 92.59(4) ?
  Pt3 Ba Al9 14_555 . . 110.666(14) ?
  Pt4 Ba Al1 . . 3_555 117.18(5) ?
  Pt4 Ba Al1 . . 22_555 117.18(5) ?
  Pt4 Ba Al2 . . 3_555 85.97(6) ?
  Pt4 Ba Al2 . . 12_555 130.10(5) ?
  Pt4 Ba Al2 . . 14_555 130.10(6) ?
  Pt4 Ba Al2 . . 22_555 85.97(4) ?
  Pt4 Ba Al3 . . 2_545 42.23(5) ?
  Pt4 Ba Al3 . . 3_665 42.23(4) ?
  Pt4 Ba Al3 . . 11_655 96.39(5) ?
  Pt4 Ba Al5 . . . 159.69(4) ?
  Pt4 Ba Al5 . . 13_655 159.69(3) ?
  Pt4 Ba Al7 . . . 42.78(6) ?
  Pt4 Ba Al8 . . . 98.04(7) ?
  Pt4 Ba Al9 . . . 36.92(2) ?
  Al1 Ba Al1 3_555 . 22_555 79.47(6) ?
  Al1 Ba Al2 3_555 . 3_555 44.83(6) ?
  Al1 Ba Al2 3_555 . 12_555 82.27(7) ?
  Al1 Ba Al2 3_555 . 14_555 111.21(8) ?
  Al1 Ba Al2 3_555 . 22_555 122.94(5) ?
  Al1 Ba Al3 3_555 . 2_545 78.85(6) ?
  Al1 Ba Al3 3_555 . 3_665 128.98(7) ?
  Al1 Ba Al3 3_555 . 11_655 124.34(5) ?
  Al1 Ba Al5 3_555 . . 75.77(6) ?
  Al1 Ba Al5 3_555 . 13_655 46.91(5) ?
  Al1 Ba Al7 3_555 . . 85.13(6) ?
  Al1 Ba Al8 3_555 . . 47.43(5) ?
  Al1 Ba Al9 3_555 . . 137.46(4) ?
  Al1 Ba Al2 22_555 . 3_555 122.94(6) ?
  Al1 Ba Al2 22_555 . 12_555 111.21(6) ?
  Al1 Ba Al2 22_555 . 14_555 82.27(5) ?
  Al1 Ba Al2 22_555 . 22_555 44.83(6) ?
  Al1 Ba Al3 22_555 . 2_545 128.98(6) ?
  Al1 Ba Al3 22_555 . 3_665 78.85(6) ?
  Al1 Ba Al3 22_555 . 11_655 124.34(5) ?
  Al1 Ba Al5 22_555 . . 46.91(5) ?
  Al1 Ba Al5 22_555 . 13_655 75.77(5) ?
  Al1 Ba Al7 22_555 . . 85.13(6) ?
  Al1 Ba Al8 22_555 . . 47.43(5) ?
  Al1 Ba Al9 22_555 . . 137.46(5) ?
  Al2 Ba Al2 3_555 . 12_555 77.71(6) ?
  Al2 Ba Al2 3_555 . 14_555 123.24(7) ?
  Al2 Ba Al2 3_555 . 22_555 157.11(5) ?
  Al2 Ba Al3 3_555 . 2_545 44.06(7) ?
  Al2 Ba Al3 3_555 . 3_665 122.84(6) ?
  Al2 Ba Al3 3_555 . 11_655 101.08(3) ?
  Al2 Ba Al5 3_555 . . 112.98(7) ?
  Al2 Ba Al5 3_555 . 13_655 73.73(6) ?
  Al2 Ba Al7 3_555 . . 79.77(4) ?
  Al2 Ba Al8 3_555 . . 79.98(4) ?
  Al2 Ba Al9 3_555 . . 93.17(5) ?
  Al2 Ba Al2 12_555 . 14_555 45.69(7) ?
  Al2 Ba Al2 12_555 . 22_555 123.24(5) ?
  Al2 Ba Al3 12_555 . 2_545 110.82(6) ?
  Al2 Ba Al3 12_555 . 3_665 148.75(8) ?
  Al2 Ba Al3 12_555 . 11_655 43.39(6) ?
  Al2 Ba Al5 12_555 . . 64.36(4) ?
  Al2 Ba Al5 12_555 . 13_655 45.70(5) ?
  Al2 Ba Al7 12_555 . . 156.98(4) ?
  Al2 Ba Al8 12_555 . . 124.24(8) ?
  Al2 Ba Al9 12_555 . . 96.83(5) ?
  Al2 Ba Al2 14_555 . 22_555 77.71(6) ?
  Al2 Ba Al3 14_555 . 2_545 148.75(6) ?
  Al2 Ba Al3 14_555 . 3_665 110.82(7) ?
  Al2 Ba Al3 14_555 . 11_655 43.39(5) ?
  Al2 Ba Al5 14_555 . . 45.70(5) ?
  Al2 Ba Al5 14_555 . 13_655 64.36(6) ?
  Al2 Ba Al7 14_555 . . 156.98(5) ?
  Al2 Ba Al8 14_555 . . 124.24(7) ?
  Al2 Ba Al9 14_555 . . 96.83(5) ?
  Al2 Ba Al3 22_555 . 2_545 122.84(6) ?
  Al2 Ba Al3 22_555 . 3_665 44.06(5) ?
  Al2 Ba Al3 22_555 . 11_655 101.08(3) ?
  Al2 Ba Al5 22_555 . . 73.73(6) ?
  Al2 Ba Al5 22_555 . 13_655 112.98(5) ?
  Al2 Ba Al7 22_555 . . 79.77(3) ?
  Al2 Ba Al8 22_555 . . 79.98(4) ?
  Al2 Ba Al9 22_555 . . 93.17(4) ?
  Al3 Ba Al3 2_545 . 3_665 80.07(6) ?
  Al3 Ba Al3 2_545 . 11_655 106.01(6) ?
  Al3 Ba Al5 2_545 . . 154.58(6) ?
  Al3 Ba Al5 2_545 . 13_655 117.58(5) ?
  Al3 Ba Al7 2_545 . . 47.49(6) ?
  Al3 Ba Al8 2_545 . . 84.88(6) ?
  Al3 Ba Al9 2_545 . . 61.64(4) ?
  Al3 Ba Al3 3_665 . 11_655 106.01(6) ?
  Al3 Ba Al5 3_665 . . 117.58(5) ?
  Al3 Ba Al5 3_665 . 13_655 154.58(5) ?
  Al3 Ba Al7 3_665 . . 47.49(5) ?
  Al3 Ba Al8 3_665 . . 84.88(7) ?
  Al3 Ba Al9 3_665 . . 61.64(5) ?
  Al3 Ba Al5 11_655 . . 87.35(4) ?
  Al3 Ba Al5 11_655 . 13_655 87.35(4) ?
  Al3 Ba Al7 11_655 . . 139.17(7) ?
  Al3 Ba Al8 11_655 . . 165.58(8) ?
  Al3 Ba Al9 11_655 . . 59.46(4) ?
  Al5 Ba Al5 . . 13_655 40.01(5) ?
  Al5 Ba Al7 . . . 130.44(5) ?
  Al5 Ba Al8 . . . 79.11(6) ?
  Al5 Ba Al9 . . . 141.71(3) ?
  Al5 Ba Al7 13_655 . . 130.44(6) ?
  Al5 Ba Al8 13_655 . . 79.11(6) ?
  Al5 Ba Al9 13_655 . . 141.708(17) ?
  Al7 Ba Al8 . . . 55.26(8) ?
  Al7 Ba Al9 . . . 79.70(6) ?
  Al8 Ba Al9 . . . 134.96(6) ?
  Ba Pt1 Pt1 . . 8_555 108.349(13) ?
  Ba Pt1 Al1 . . 3_555 61.19(8) ?
  Ba Pt1 Al1 . . 22_555 61.19(4) ?
  Ba Pt1 Al2 . . 2_655 138.59(4) ?
  Ba Pt1 Al2 . . 24_655 138.59(6) ?
  Ba Pt1 Al4 . . 2_655 122.80(6) ?
  Ba Pt1 Al4 . . 9_655 122.80(11) ?
  Ba Pt1 Al5 . . . 73.65(4) ?
  Ba Pt1 Al5 . . 13_655 73.65(5) ?
  Ba Pt1 Al8 . . . 59.86(6) ?
  Pt1 Pt1 Al1 8_555 . 3_555 84.55(5) ?
  Pt1 Pt1 Al1 8_555 . 22_555 84.55(5) ?
  Pt1 Pt1 Al2 8_555 . 2_655 100.34(5) ?
  Pt1 Pt1 Al2 8_555 . 24_655 100.34(4) ?
  Pt1 Pt1 Al4 8_555 . 2_655 46.91(7) ?
  Pt1 Pt1 Al4 8_555 . 9_655 46.91(5) ?
  Pt1 Pt1 Al5 8_555 . . 149.07(5) ?
  Pt1 Pt1 Al5 8_555 . 13_655 149.07(5) ?
  Pt1 Pt1 Al8 8_555 . . 48.49(6) ?
  Al1 Pt1 Al1 3_555 . 22_555 113.61(9) ?
  Al1 Pt1 Al2 3_555 . 2_655 93.47(9) ?
  Al1 Pt1 Al2 3_555 . 24_655 152.87(11) ?
  Al1 Pt1 Al4 3_555 . 2_655 65.26(9) ?
  Al1 Pt1 Al4 3_555 . 9_655 131.27(7) ?
  Al1 Pt1 Al5 3_555 . . 120.33(6) ?
  Al1 Pt1 Al5 3_555 . 13_655 69.20(6) ?
  Al1 Pt1 Al8 3_555 . . 62.18(7) ?
  Al1 Pt1 Al2 22_555 . 2_655 152.87(6) ?
  Al1 Pt1 Al2 22_555 . 24_655 93.47(9) ?
  Al1 Pt1 Al4 22_555 . 2_655 131.27(9) ?
  Al1 Pt1 Al4 22_555 . 9_655 65.26(12) ?
  Al1 Pt1 Al5 22_555 . . 69.20(8) ?
  Al1 Pt1 Al5 22_555 . 13_655 120.33(8) ?
  Al1 Pt1 Al8 22_555 . . 62.18(5) ?
  Al2 Pt1 Al2 2_655 . 24_655 59.43(9) ?
  Al2 Pt1 Al4 2_655 . 2_655 60.72(9) ?
  Al2 Pt1 Al4 2_655 . 9_655 98.60(12) ?
  Al2 Pt1 Al5 2_655 . . 96.38(8) ?
  Al2 Pt1 Al5 2_655 . 13_655 66.52(7) ?
  Al2 Pt1 Al8 2_655 . . 139.05(6) ?
  Al2 Pt1 Al4 24_655 . 2_655 98.60(9) ?
  Al2 Pt1 Al4 24_655 . 9_655 60.72(8) ?
  Al2 Pt1 Al5 24_655 . . 66.52(6) ?
  Al2 Pt1 Al5 24_655 . 13_655 96.38(6) ?
  Al2 Pt1 Al8 24_655 . . 139.05(7) ?
  Al4 Pt1 Al4 2_655 . 9_655 80.21(11) ?
  Al4 Pt1 Al5 2_655 . . 157.10(10) ?
  Al4 Pt1 Al5 2_655 . 13_655 105.02(9) ?
  Al4 Pt1 Al8 2_655 . . 78.75(9) ?
  Al4 Pt1 Al5 9_655 . . 105.02(7) ?
  Al4 Pt1 Al5 9_655 . 13_655 157.10(7) ?
  Al4 Pt1 Al8 9_655 . . 78.75(9) ?
  Al5 Pt1 Al5 . . 13_655 61.84(7) ?
  Al5 Pt1 Al8 . . . 124.02(7) ?
  Al5 Pt1 Al8 13_655 . . 124.02(6) ?
  Ba Pt2 Ba 2_555 . 7_555 109.941(13) ?
  Ba Pt2 Al1 2_555 . . 63.88(4) ?
  Ba Pt2 Al1 2_555 . 16_555 120.66(6) ?
  Ba Pt2 Al2 2_555 . . 67.99(4) ?
  Ba Pt2 Al2 2_555 . 16_555 177.02(4) ?
  Ba Pt2 Al3 2_555 . 3_665 67.05(7) ?
  Ba Pt2 Al3 2_555 . 9_665 117.26(6) ?
  Ba Pt2 Al4 2_555 . . 122.84(2) ?
  Ba Pt2 Al7 2_555 . 2_555 62.12(3) ?
  Ba Pt2 Al8 2_555 . 2_555 63.14(3) ?
  Ba Pt2 Al1 7_555 . . 120.66(6) ?
  Ba Pt2 Al1 7_555 . 16_555 63.88(4) ?
  Ba Pt2 Al2 7_555 . . 177.02(4) ?
  Ba Pt2 Al2 7_555 . 16_555 67.99(4) ?
  Ba Pt2 Al3 7_555 . 3_665 117.26(6) ?
  Ba Pt2 Al3 7_555 . 9_665 67.05(7) ?
  Ba Pt2 Al4 7_555 . . 122.84(2) ?
  Ba Pt2 Al7 7_555 . 2_555 62.12(3) ?
  Ba Pt2 Al8 7_555 . 2_555 63.14(3) ?
  Al1 Pt2 Al1 . . 16_555 70.92(7) ?
  Al1 Pt2 Al2 . . . 60.71(8) ?
  Al1 Pt2 Al2 . . 16_555 118.93(6) ?
  Al1 Pt2 Al3 . . 3_665 112.91(8) ?
  Al1 Pt2 Al3 . . 9_665 171.89(8) ?
  Al1 Pt2 Al4 . . . 71.14(8) ?
  Al1 Pt2 Al7 . . 2_555 121.37(7) ?
  Al1 Pt2 Al8 . . 2_555 63.06(8) ?
  Al1 Pt2 Al2 16_555 . . 118.93(6) ?
  Al1 Pt2 Al2 16_555 . 16_555 60.71(8) ?
  Al1 Pt2 Al3 16_555 . 3_665 171.89(8) ?
  Al1 Pt2 Al3 16_555 . 9_665 112.91(8) ?
  Al1 Pt2 Al4 16_555 . . 71.14(8) ?
  Al1 Pt2 Al7 16_555 . 2_555 121.37(7) ?
  Al1 Pt2 Al8 16_555 . 2_555 63.06(8) ?
  Al2 Pt2 Al2 . . 16_555 113.98(6) ?
  Al2 Pt2 Al3 . . 3_665 60.12(8) ?
  Al2 Pt2 Al3 . . 9_665 111.73(9) ?
  Al2 Pt2 Al4 . . . 59.91(4) ?
  Al2 Pt2 Al7 . . 2_555 114.91(5) ?
  Al2 Pt2 Al8 . . 2_555 116.79(6) ?
  Al2 Pt2 Al3 16_555 . 3_665 111.73(9) ?
  Al2 Pt2 Al3 16_555 . 9_665 60.12(8) ?
  Al2 Pt2 Al4 16_555 . . 59.91(4) ?
  Al2 Pt2 Al7 16_555 . 2_555 114.91(5) ?
  Al2 Pt2 Al8 16_555 . 2_555 116.79(6) ?
  Al3 Pt2 Al3 3_665 . 9_665 62.37(9) ?
  Al3 Pt2 Al4 3_665 . . 102.90(9) ?
  Al3 Pt2 Al7 3_665 . 2_555 63.47(7) ?
  Al3 Pt2 Al8 3_665 . 2_555 124.96(8) ?
  Al3 Pt2 Al4 9_665 . . 102.90(9) ?
  Al3 Pt2 Al7 9_665 . 2_555 63.47(7) ?
  Al3 Pt2 Al8 9_665 . 2_555 124.96(8) ?
  Al4 Pt2 Al7 . . 2_555 163.66(11) ?
  Al4 Pt2 Al8 . . 2_555 122.81(11) ?
  Al7 Pt2 Al8 2_555 . 2_555 73.53(10) ?
  Ba Pt3 Ba 2_555 . 12_555 70.788(14) ?
  Ba Pt3 Pt3 2_555 . 2_665 162.634(9) ?
  Ba Pt3 Pt3 2_555 . 3_565 117.228(14) ?
  Ba Pt3 Al1 2_555 . . 63.85(4) ?
  Ba Pt3 Al1 2_555 . 11_555 118.55(4) ?
  Ba Pt3 Al2 2_555 . . 70.18(4) ?
  Ba Pt3 Al2 2_555 . 11_555 64.90(5) ?
  Ba Pt3 Al5 2_555 . 14_565 78.48(5) ?
  Ba Pt3 Al5 2_555 . 15_555 137.58(4) ?
  Ba Pt3 Al6 2_555 . . 122.88(5) ?
  Ba Pt3 Al6 2_555 . 10_665 148.36(2) ?
  Ba Pt3 Pt3 12_555 . 2_665 117.228(14) ?
  Ba Pt3 Pt3 12_555 . 3_565 162.634(9) ?
  Ba Pt3 Al1 12_555 . . 118.55(5) ?
  Ba Pt3 Al1 12_555 . 11_555 63.85(5) ?
  Ba Pt3 Al2 12_555 . . 64.90(5) ?
  Ba Pt3 Al2 12_555 . 11_555 70.18(8) ?
  Ba Pt3 Al5 12_555 . 14_565 137.58(5) ?
  Ba Pt3 Al5 12_555 . 15_555 78.48(4) ?
  Ba Pt3 Al6 12_555 . . 148.36(2) ?
  Ba Pt3 Al6 12_555 . 10_665 122.88(5) ?
  Pt3 Pt3 Pt3 2_665 . 3_565 60.000(13) ?
  Pt3 Pt3 Al1 2_665 . . 99.45(4) ?
  Pt3 Pt3 Al1 2_665 . 11_555 78.26(4) ?
  Pt3 Pt3 Al2 2_665 . . 98.49(4) ?
  Pt3 Pt3 Al2 2_665 . 11_555 131.54(4) ?
  Pt3 Pt3 Al5 2_665 . 14_565 100.71(6) ?
  Pt3 Pt3 Al5 2_665 . 15_555 40.71(4) ?
  Pt3 Pt3 Al6 2_665 . . 42.22(4) ?
  Pt3 Pt3 Al6 2_665 . 10_665 42.22(4) ?
  Pt3 Pt3 Al1 3_565 . . 78.26(5) ?
  Pt3 Pt3 Al1 3_565 . 11_555 99.45(6) ?
  Pt3 Pt3 Al2 3_565 . . 131.54(5) ?
  Pt3 Pt3 Al2 3_565 . 11_555 98.49(7) ?
  Pt3 Pt3 Al5 3_565 . 14_565 40.71(5) ?
  Pt3 Pt3 Al5 3_565 . 15_555 100.71(4) ?
  Pt3 Pt3 Al6 3_565 . . 42.22(4) ?
  Pt3 Pt3 Al6 3_565 . 10_665 42.22(4) ?
  Al1 Pt3 Al1 . . 11_555 177.39(6) ?
  Al1 Pt3 Al2 . . . 62.15(8) ?
  Al1 Pt3 Al2 . . 11_555 119.24(8) ?
  Al1 Pt3 Al5 . . 14_565 69.24(6) ?
  Al1 Pt3 Al5 . . 15_555 109.84(5) ?
  Al1 Pt3 Al6 . . . 59.91(7) ?
  Al1 Pt3 Al6 . . 10_665 117.54(7) ?
  Al1 Pt3 Al2 11_555 . . 119.24(9) ?
  Al1 Pt3 Al2 11_555 . 11_555 62.15(8) ?
  Al1 Pt3 Al5 11_555 . 14_565 109.84(7) ?
  Al1 Pt3 Al5 11_555 . 15_555 69.24(6) ?
  Al1 Pt3 Al6 11_555 . . 117.54(7) ?
  Al1 Pt3 Al6 11_555 . 10_665 59.91(7) ?
  Al2 Pt3 Al2 . . 11_555 124.17(7) ?
  Al2 Pt3 Al5 . . 14_565 129.88(6) ?
  Al2 Pt3 Al5 . . 15_555 70.61(5) ?
  Al2 Pt3 Al6 . . . 91.63(7) ?
  Al2 Pt3 Al6 . . 10_665 140.57(5) ?
  Al2 Pt3 Al5 11_555 . 14_565 70.61(9) ?
  Al2 Pt3 Al5 11_555 . 15_555 129.88(7) ?
  Al2 Pt3 Al6 11_555 . . 140.57(8) ?
  Al2 Pt3 Al6 11_555 . 10_665 91.63(7) ?
  Al5 Pt3 Al5 14_565 . 15_555 141.43(7) ?
  Al5 Pt3 Al6 14_565 . . 73.59(5) ?
  Al5 Pt3 Al6 14_565 . 10_665 73.59(5) ?
  Al5 Pt3 Al6 15_555 . . 73.59(4) ?
  Al5 Pt3 Al6 15_555 . 10_665 73.59(4) ?
  Al6 Pt3 Al6 . . 10_665 62.44(9) ?
  Ba Pt4 Ba . . 2_555 108.68(3) ?
  Ba Pt4 Ba . . 3_555 108.68(3) ?
  Ba Pt4 Pt4 . . 7_555 110.25(3) ?
  Ba Pt4 Al3 . . 1_455 165.17(9) ?
  Ba Pt4 Al3 . . 2_545 64.26(3) ?
  Ba Pt4 Al3 . . 3_665 64.26(7) ?
  Ba Pt4 Al7 . . . 58.91(5) ?
  Ba Pt4 Al7 . . 2_555 125.628(16) ?
  Ba Pt4 Al7 . . 3_555 125.63(10) ?
  Ba Pt4 Al9 . . . 69.75(3) ?
  Ba Pt4 Ba 2_555 . 3_555 108.68(3) ?
  Ba Pt4 Pt4 2_555 . 7_555 110.25(3) ?
  Ba Pt4 Al3 2_555 . 1_455 64.26(3) ?
  Ba Pt4 Al3 2_555 . 2_545 165.17(9) ?
  Ba Pt4 Al3 2_555 . 3_665 64.26(7) ?
  Ba Pt4 Al7 2_555 . . 125.628(16) ?
  Ba Pt4 Al7 2_555 . 2_555 58.91(5) ?
  Ba Pt4 Al7 2_555 . 3_555 125.63(10) ?
  Ba Pt4 Al9 2_555 . . 69.75(3) ?
  Ba Pt4 Pt4 3_555 . 7_555 110.25(3) ?
  Ba Pt4 Al3 3_555 . 1_455 64.26(3) ?
  Ba Pt4 Al3 3_555 . 2_545 64.26(3) ?
  Ba Pt4 Al3 3_555 . 3_665 165.17(9) ?
  Ba Pt4 Al7 3_555 . . 125.628(18) ?
  Ba Pt4 Al7 3_555 . 2_555 125.628(18) ?
  Ba Pt4 Al7 3_555 . 3_555 58.91(4) ?
  Ba Pt4 Al9 3_555 . . 69.75(3) ?
  Pt4 Pt4 Al3 7_555 . 1_455 84.58(8) ?
  Pt4 Pt4 Al3 7_555 . 2_545 84.58(8) ?
  Pt4 Pt4 Al3 7_555 . 3_665 84.58(8) ?
  Pt4 Pt4 Al7 7_555 . . 51.34(6) ?
  Pt4 Pt4 Al7 7_555 . 2_555 51.34(6) ?
  Pt4 Pt4 Al7 7_555 . 3_555 51.34(5) ?
  Pt4 Pt4 Al9 7_555 . . 180 ?
  Al3 Pt4 Al3 1_455 . 2_545 119.12(2) ?
  Al3 Pt4 Al3 1_455 . 3_665 119.12(8) ?
  Al3 Pt4 Al7 1_455 . . 135.92(11) ?
  Al3 Pt4 Al7 1_455 . 2_555 63.41(5) ?
  Al3 Pt4 Al7 1_455 . 3_555 63.41(11) ?
  Al3 Pt4 Al9 1_455 . . 95.42(8) ?
  Al3 Pt4 Al3 2_545 . 3_665 119.12(8) ?
  Al3 Pt4 Al7 2_545 . . 63.41(5) ?
  Al3 Pt4 Al7 2_545 . 2_555 135.92(11) ?
  Al3 Pt4 Al7 2_545 . 3_555 63.41(11) ?
  Al3 Pt4 Al9 2_545 . . 95.42(8) ?
  Al3 Pt4 Al7 3_665 . . 63.41(7) ?
  Al3 Pt4 Al7 3_665 . 2_555 63.41(7) ?
  Al3 Pt4 Al7 3_665 . 3_555 135.92(10) ?
  Al3 Pt4 Al9 3_665 . . 95.42(8) ?
  Al7 Pt4 Al7 . . 2_555 85.10(7) ?
  Al7 Pt4 Al7 . . 3_555 85.10(9) ?
  Al7 Pt4 Al9 . . . 128.66(6) ?
  Al7 Pt4 Al7 2_555 . 3_555 85.10(9) ?
  Al7 Pt4 Al9 2_555 . . 128.66(6) ?
  Al7 Pt4 Al9 3_555 . . 128.66(5) ?
  Al1 Pt5 Al1 . . 2_665 93.59(7) ?
  Al1 Pt5 Al1 . . 3_565 93.59(7) ?
  Al1 Pt5 Al1 . . 16_555 65.37(6) ?
  Al1 Pt5 Al1 . . 17_665 130.23(9) ?
  Al1 Pt5 Al1 . . 18_565 130.23(8) ?
  Al1 Pt5 Al4 . . . 68.35(8) ?
  Al1 Pt5 Al4 . . 2_665 147.10(4) ?
  Al1 Pt5 Al4 . . 3_565 61.92(8) ?
  Al1 Pt5 Al6 . . . 57.31(4) ?
  Al1 Pt5 Al6 . . 16_555 122.69(4) ?
  Al1 Pt5 Al1 2_665 . 3_565 93.59(9) ?
  Al1 Pt5 Al1 2_665 . 16_555 130.23(9) ?
  Al1 Pt5 Al1 2_665 . 17_665 65.37(7) ?
  Al1 Pt5 Al1 2_665 . 18_565 130.23(7) ?
  Al1 Pt5 Al4 2_665 . . 61.92(8) ?
  Al1 Pt5 Al4 2_665 . 2_665 68.35(10) ?
  Al1 Pt5 Al4 2_665 . 3_565 147.10(5) ?
  Al1 Pt5 Al6 2_665 . . 57.31(5) ?
  Al1 Pt5 Al6 2_665 . 16_555 122.69(5) ?
  Al1 Pt5 Al1 3_565 . 16_555 130.23(8) ?
  Al1 Pt5 Al1 3_565 . 17_665 130.23(7) ?
  Al1 Pt5 Al1 3_565 . 18_565 65.37(7) ?
  Al1 Pt5 Al4 3_565 . . 147.10(5) ?
  Al1 Pt5 Al4 3_565 . 2_665 61.92(9) ?
  Al1 Pt5 Al4 3_565 . 3_565 68.35(9) ?
  Al1 Pt5 Al6 3_565 . . 57.31(5) ?
  Al1 Pt5 Al6 3_565 . 16_555 122.69(5) ?
  Al1 Pt5 Al1 16_555 . 17_665 93.59(7) ?
  Al1 Pt5 Al1 16_555 . 18_565 93.59(7) ?
  Al1 Pt5 Al4 16_555 . . 68.35(8) ?
  Al1 Pt5 Al4 16_555 . 2_665 147.10(4) ?
  Al1 Pt5 Al4 16_555 . 3_565 61.92(8) ?
  Al1 Pt5 Al6 16_555 . . 122.69(4) ?
  Al1 Pt5 Al6 16_555 . 16_555 57.31(4) ?
  Al1 Pt5 Al1 17_665 . 18_565 93.59(9) ?
  Al1 Pt5 Al4 17_665 . . 61.92(8) ?
  Al1 Pt5 Al4 17_665 . 2_665 68.35(10) ?
  Al1 Pt5 Al4 17_665 . 3_565 147.10(5) ?
  Al1 Pt5 Al6 17_665 . . 122.69(5) ?
  Al1 Pt5 Al6 17_665 . 16_555 57.31(5) ?
  Al1 Pt5 Al4 18_565 . . 147.10(5) ?
  Al1 Pt5 Al4 18_565 . 2_665 61.92(9) ?
  Al1 Pt5 Al4 18_565 . 3_565 68.35(9) ?
  Al1 Pt5 Al6 18_565 . . 122.69(5) ?
  Al1 Pt5 Al6 18_565 . 16_555 57.31(5) ?
  Al4 Pt5 Al4 . . 2_665 120.00(12) ?
  Al4 Pt5 Al4 . . 3_565 120.00(10) ?
  Al4 Pt5 Al6 . . . 90 ?
  Al4 Pt5 Al6 . . 16_555 90 ?
  Al4 Pt5 Al4 2_665 . 3_565 120.00(13) ?
  Al4 Pt5 Al6 2_665 . . 90 ?
  Al4 Pt5 Al6 2_665 . 16_555 90 ?
  Al4 Pt5 Al6 3_565 . . 90 ?
  Al4 Pt5 Al6 3_565 . 16_555 90 ?
  Al6 Pt5 Al6 . . 16_555 180 ?
  Ba Al1 Pt1 2_555 . 2_555 76.79(5) ?
  Ba Al1 Pt2 2_555 . . 72.37(5) ?
  Ba Al1 Pt3 2_555 . . 70.90(5) ?
  Ba Al1 Pt5 2_555 . . 168.45(10) ?
  Ba Al1 Al1 2_555 . 16_555 114.98(6) ?
  Ba Al1 Al2 2_555 . . 71.49(6) ?
  Ba Al1 Al2 2_555 . 3_565 112.97(7) ?
  Ba Al1 Al4 2_555 . . 116.72(10) ?
  Ba Al1 Al4 2_555 . 3_565 129.79(11) ?
  Ba Al1 Al5 2_555 . 14_565 76.30(7) ?
  Ba Al1 Al6 2_555 . . 128.03(10) ?
  Ba Al1 Al8 2_555 . 2_555 65.43(6) ?
  Pt1 Al1 Pt2 2_555 . . 117.45(7) ?
  Pt1 Al1 Pt3 2_555 . . 106.16(8) ?
  Pt1 Al1 Pt5 2_555 . . 111.33(9) ?
  Pt1 Al1 Al1 2_555 . 16_555 95.45(9) ?
  Pt1 Al1 Al2 2_555 . . 147.06(9) ?
  Pt1 Al1 Al2 2_555 . 3_565 43.79(6) ?
  Pt1 Al1 Al4 2_555 . . 155.00(10) ?
  Pt1 Al1 Al4 2_555 . 3_565 57.16(10) ?
  Pt1 Al1 Al5 2_555 . 14_565 55.89(8) ?
  Pt1 Al1 Al6 2_555 . . 106.95(9) ?
  Pt1 Al1 Al8 2_555 . 2_555 60.13(8) ?
  Pt2 Al1 Pt3 . . . 112.70(10) ?
  Pt2 Al1 Pt5 . . . 96.28(7) ?
  Pt2 Al1 Al1 . . 16_555 54.54(6) ?
  Pt2 Al1 Al2 . . . 60.65(7) ?
  Pt2 Al1 Al2 . . 3_565 151.45(9) ?
  Pt2 Al1 Al4 . . . 54.53(7) ?
  Pt2 Al1 Al4 . . 3_565 110.13(9) ?
  Pt2 Al1 Al5 . . 14_565 148.57(9) ?
  Pt2 Al1 Al6 . . . 134.93(11) ?
  Pt2 Al1 Al8 . . 2_555 57.74(8) ?
  Pt3 Al1 Pt5 . . . 112.97(7) ?
  Pt3 Al1 Al1 . . 16_555 158.39(12) ?
  Pt3 Al1 Al2 . . . 55.04(7) ?
  Pt3 Al1 Al2 . . 3_565 95.04(7) ?
  Pt3 Al1 Al4 . . . 98.38(9) ?
  Pt3 Al1 Al4 . . 3_565 136.72(10) ?
  Pt3 Al1 Al5 . . 14_565 52.79(7) ?
  Pt3 Al1 Al6 . . . 58.09(7) ?
  Pt3 Al1 Al8 . . 2_555 136.11(8) ?
  Pt5 Al1 Al1 . . 16_555 57.31(5) ?
  Pt5 Al1 Al2 . . . 101.37(9) ?
  Pt5 Al1 Al2 . . 3_565 77.99(6) ?
  Pt5 Al1 Al4 . . . 52.64(7) ?
  Pt5 Al1 Al4 . . 3_565 55.44(9) ?
  Pt5 Al1 Al5 . . 14_565 114.92(9) ?
  Pt5 Al1 Al6 . . . 58.80(7) ?
  Pt5 Al1 Al8 . . 2_555 110.72(9) ?
  Al1 Al1 Al2 16_555 . . 105.67(11) ?
  Al1 Al1 Al2 16_555 . 3_565 100.90(9) ?
  Al1 Al1 Al4 16_555 . . 60.13(8) ?
  Al1 Al1 Al4 16_555 . 3_565 57.07(9) ?
  Al1 Al1 Al5 16_555 . 14_565 147.45(13) ?
  Al1 Al1 Al6 16_555 . . 116.11(9) ?
  Al1 Al1 Al8 16_555 . 2_555 56.01(6) ?
  Al2 Al1 Al2 . . 3_565 147.78(9) ?
  Al2 Al1 Al4 . . . 54.58(8) ?
  Al2 Al1 Al4 . . 3_565 155.53(13) ?
  Al2 Al1 Al5 . . 14_565 106.88(11) ?
  Al2 Al1 Al6 . . . 86.33(8) ?
  Al2 Al1 Al8 . . 2_555 112.08(12) ?
  Al2 Al1 Al4 3_565 . . 130.23(8) ?
  Al2 Al1 Al4 3_565 . 3_565 43.84(7) ?
  Al2 Al1 Al5 3_565 . 14_565 48.50(8) ?
  Al2 Al1 Al6 3_565 . . 65.54(6) ?
  Al2 Al1 Al8 3_565 . 2_555 97.74(12) ?
  Al4 Al1 Al4 . . 3_565 101.15(11) ?
  Al4 Al1 Al5 . . 14_565 144.70(9) ?
  Al4 Al1 Al6 . . . 81.88(8) ?
  Al4 Al1 Al8 . . 2_555 104.61(9) ?
  Al4 Al1 Al5 3_565 . 14_565 91.71(12) ?
  Al4 Al1 Al6 3_565 . . 86.97(9) ?
  Al4 Al1 Al8 3_565 . 2_555 74.34(11) ?
  Al5 Al1 Al6 14_565 . . 65.98(8) ?
  Al5 Al1 Al8 14_565 . 2_555 110.51(10) ?
  Al6 Al1 Al8 . . 2_555 161.03(14) ?
  Ba Al2 Ba 2_555 . 12_555 72.84(4) ?
  Ba Al2 Pt1 2_555 . 3_665 178.89(8) ?
  Ba Al2 Pt2 2_555 . . 68.46(4) ?
  Ba Al2 Pt3 2_555 . . 69.41(5) ?
  Ba Al2 Al1 2_555 . . 63.68(6) ?
  Ba Al2 Al1 2_555 . 2_665 137.49(10) ?
  Ba Al2 Al2 2_555 . 22_555 119.44(7) ?
  Ba Al2 Al3 2_555 . 3_665 67.27(7) ?
  Ba Al2 Al4 2_555 . . 122.59(11) ?
  Ba Al2 Al4 2_555 . 7_555 140.51(7) ?
  Ba Al2 Al5 2_555 . 3_665 137.32(6) ?
  Ba Al2 Al5 2_555 . 15_555 122.70(9) ?
  Ba Al2 Al6 2_555 . . 97.52(7) ?
  Ba Al2 Pt1 12_555 . 3_665 106.15(8) ?
  Ba Al2 Pt2 12_555 . . 130.23(6) ?
  Ba Al2 Pt3 12_555 . . 73.50(5) ?
  Ba Al2 Al1 12_555 . . 126.17(9) ?
  Ba Al2 Al1 12_555 . 2_665 127.31(6) ?
  Ba Al2 Al2 12_555 . 22_555 67.16(7) ?
  Ba Al2 Al3 12_555 . 3_665 76.74(8) ?
  Ba Al2 Al4 12_555 . . 163.33(13) ?
  Ba Al2 Al4 12_555 . 7_555 108.23(8) ?
  Ba Al2 Al5 12_555 . 3_665 64.83(4) ?
  Ba Al2 Al5 12_555 . 15_555 77.55(5) ?
  Ba Al2 Al6 12_555 . . 115.67(8) ?
  Pt1 Al2 Pt2 3_665 . . 112.64(7) ?
  Pt1 Al2 Pt3 3_665 . . 109.92(7) ?
  Pt1 Al2 Al1 3_665 . . 116.90(8) ?
  Pt1 Al2 Al1 3_665 . 2_665 42.75(6) ?
  Pt1 Al2 Al2 3_665 . 22_555 60.29(7) ?
  Pt1 Al2 Al3 3_665 . 3_665 113.07(12) ?
  Pt1 Al2 Al4 3_665 . . 58.47(8) ?
  Pt1 Al2 Al4 3_665 . 7_555 40.11(5) ?
  Pt1 Al2 Al5 3_665 . 3_665 41.62(4) ?
  Pt1 Al2 Al5 3_665 . 15_555 56.41(6) ?
  Pt1 Al2 Al6 3_665 . . 82.47(5) ?
  Pt2 Al2 Pt3 . . . 118.11(11) ?
  Pt2 Al2 Al1 . . . 58.64(7) ?
  Pt2 Al2 Al1 . . 2_665 102.43(7) ?
  Pt2 Al2 Al2 . . 22_555 106.97(9) ?
  Pt2 Al2 Al3 . . 3_665 60.23(8) ?
  Pt2 Al2 Al4 . . . 59.15(7) ?
  Pt2 Al2 Al4 . . 7_555 84.44(6) ?
  Pt2 Al2 Al5 . . 3_665 147.56(9) ?
  Pt2 Al2 Al5 . . 15_555 150.98(9) ?
  Pt2 Al2 Al6 . . . 99.54(9) ?
  Pt3 Al2 Al1 . . . 62.81(8) ?
  Pt3 Al2 Al1 . . 2_665 80.86(7) ?
  Pt3 Al2 Al2 . . 22_555 132.88(10) ?
  Pt3 Al2 Al3 . . 3_665 132.82(10) ?
  Pt3 Al2 Al4 . . . 116.19(12) ?
  Pt3 Al2 Al4 . . 7_555 149.94(7) ?
  Pt3 Al2 Al5 . . 3_665 92.89(6) ?
  Pt3 Al2 Al5 . . 15_555 55.48(7) ?
  Pt3 Al2 Al6 . . . 45.38(6) ?
  Al1 Al2 Al1 . . 2_665 76.05(8) ?
  Al1 Al2 Al2 . . 22_555 164.24(11) ?
  Al1 Al2 Al3 . . 3_665 111.23(11) ?
  Al1 Al2 Al4 . . . 69.96(12) ?
  Al1 Al2 Al4 . . 7_555 125.41(9) ?
  Al1 Al2 Al5 . . 3_665 142.21(8) ?
  Al1 Al2 Al5 . . 15_555 100.11(10) ?
  Al1 Al2 Al6 . . . 46.40(6) ?
  Al1 Al2 Al2 2_665 . 22_555 103.03(8) ?
  Al1 Al2 Al3 2_665 . 3_665 145.83(10) ?
  Al1 Al2 Al4 2_665 . . 47.02(6) ?
  Al1 Al2 Al4 2_665 . 7_555 74.61(7) ?
  Al1 Al2 Al5 2_665 . 3_665 71.55(6) ?
  Al1 Al2 Al5 2_665 . 15_555 50.18(5) ?
  Al1 Al2 Al6 2_665 . . 41.34(6) ?
  Al2 Al2 Al3 22_555 . 3_665 60.74(10) ?
  Al2 Al2 Al4 22_555 . . 97.66(12) ?
  Al2 Al2 Al4 22_555 . 7_555 41.36(7) ?
  Al2 Al2 Al5 22_555 . 3_665 47.38(6) ?
  Al2 Al2 Al5 22_555 . 15_555 90.75(10) ?
  Al2 Al2 Al6 22_555 . . 140.24(7) ?
  Al3 Al2 Al4 3_665 . . 102.43(11) ?
  Al3 Al2 Al4 3_665 . 7_555 74.53(9) ?
  Al3 Al2 Al5 3_665 . 3_665 106.50(11) ?
  Al3 Al2 Al5 3_665 . 15_555 147.36(13) ?
  Al3 Al2 Al6 3_665 . . 157.60(12) ?
  Al4 Al2 Al4 . . 7_555 56.30(11) ?
  Al4 Al2 Al5 . . 3_665 100.09(9) ?
  Al4 Al2 Al5 . . 15_555 96.52(7) ?
  Al4 Al2 Al6 . . . 71.14(10) ?
  Al4 Al2 Al5 7_555 . 3_665 63.15(5) ?
  Al4 Al2 Al5 7_555 . 15_555 94.98(8) ?
  Al4 Al2 Al6 7_555 . . 115.45(7) ?
  Al5 Al2 Al5 3_665 . 15_555 43.38(7) ?
  Al5 Al2 Al6 3_665 . . 95.83(5) ?
  Al5 Al2 Al6 15_555 . . 54.58(7) ?
  Ba Al3 Ba 2_655 . 3_655 119.75(9) ?
  Ba Al3 Ba 2_655 . 11_655 68.42(5) ?
  Ba Al3 Pt2 2_655 . 2_655 170.73(9) ?
  Ba Al3 Pt2 2_655 . 9_655 68.918(15) ?
  Ba Al3 Pt4 2_655 . 1_655 73.51(5) ?
  Ba Al3 Al2 2_655 . 2_655 118.80(11) ?
  Ba Al3 Al2 2_655 . 24_655 68.67(5) ?
  Ba Al3 Al3 2_655 . 8_555 116.03(5) ?
  Ba Al3 Al7 2_655 . 2_655 61.61(5) ?
  Ba Al3 Al7 2_655 . 3_655 129.17(11) ?
  Ba Al3 Al9 2_655 . 1_655 61.18(4) ?
  Ba Al3 Ba 3_655 . 11_655 68.42(5) ?
  Ba Al3 Pt2 3_655 . 2_655 68.918(16) ?
  Ba Al3 Pt2 3_655 . 9_655 170.73(9) ?
  Ba Al3 Pt4 3_655 . 1_655 73.51(5) ?
  Ba Al3 Al2 3_655 . 2_655 68.67(8) ?
  Ba Al3 Al2 3_655 . 24_655 118.80(10) ?
  Ba Al3 Al3 3_655 . 8_555 116.03(5) ?
  Ba Al3 Al7 3_655 . 2_655 129.17(12) ?
  Ba Al3 Al7 3_655 . 3_655 61.61(5) ?
  Ba Al3 Al9 3_655 . 1_655 61.18(4) ?
  Ba Al3 Pt2 11_655 . 2_655 114.69(7) ?
  Ba Al3 Pt2 11_655 . 9_655 114.69(7) ?
  Ba Al3 Pt4 11_655 . 1_655 98.44(9) ?
  Ba Al3 Al2 11_655 . 2_655 59.87(7) ?
  Ba Al3 Al2 11_655 . 24_655 59.87(7) ?
  Ba Al3 Al3 11_655 . 8_555 166.14(12) ?
  Ba Al3 Al7 11_655 . 2_655 128.75(7) ?
  Ba Al3 Al7 11_655 . 3_655 128.75(8) ?
  Ba Al3 Al9 11_655 . 1_655 59.05(5) ?
  Pt2 Al3 Pt2 2_655 . 9_655 102.24(10) ?
  Pt2 Al3 Pt4 2_655 . 1_655 113.71(8) ?
  Pt2 Al3 Al2 2_655 . 2_655 59.66(7) ?
  Pt2 Al3 Al2 2_655 . 24_655 104.82(10) ?
  Pt2 Al3 Al3 2_655 . 8_555 58.82(6) ?
  Pt2 Al3 Al7 2_655 . 2_655 116.46(11) ?
  Pt2 Al3 Al7 2_655 . 3_655 56.57(7) ?
  Pt2 Al3 Al9 2_655 . 1_655 128.07(5) ?
  Pt2 Al3 Pt4 9_655 . 1_655 113.71(8) ?
  Pt2 Al3 Al2 9_655 . 2_655 104.82(12) ?
  Pt2 Al3 Al2 9_655 . 24_655 59.66(6) ?
  Pt2 Al3 Al3 9_655 . 8_555 58.82(6) ?
  Pt2 Al3 Al7 9_655 . 2_655 56.57(8) ?
  Pt2 Al3 Al7 9_655 . 3_655 116.46(12) ?
  Pt2 Al3 Al9 9_655 . 1_655 128.07(5) ?
  Pt4 Al3 Al2 1_655 . 2_655 141.22(11) ?
  Pt4 Al3 Al2 1_655 . 24_655 141.22(10) ?
  Pt4 Al3 Al3 1_655 . 8_555 95.42(12) ?
  Pt4 Al3 Al7 1_655 . 2_655 57.81(8) ?
  Pt4 Al3 Al7 1_655 . 3_655 57.81(9) ?
  Pt4 Al3 Al9 1_655 . 1_655 39.40(5) ?
  Al2 Al3 Al2 2_655 . 24_655 58.52(10) ?
  Al2 Al3 Al3 2_655 . 8_555 108.44(11) ?
  Al2 Al3 Al7 2_655 . 2_655 160.91(14) ?
  Al2 Al3 Al7 2_655 . 3_655 108.62(9) ?
  Al2 Al3 Al9 2_655 . 1_655 110.72(10) ?
  Al2 Al3 Al3 24_655 . 8_555 108.44(11) ?
  Al2 Al3 Al7 24_655 . 2_655 108.62(9) ?
  Al2 Al3 Al7 24_655 . 3_655 160.91(13) ?
  Al2 Al3 Al9 24_655 . 1_655 110.72(10) ?
  Al3 Al3 Al7 8_555 . 2_655 59.94(7) ?
  Al3 Al3 Al7 8_555 . 3_655 59.94(8) ?
  Al3 Al3 Al9 8_555 . 1_655 134.82(11) ?
  Al7 Al3 Al7 2_655 . 3_655 79.58(12) ?
  Al7 Al3 Al9 2_655 . 1_655 86.55(7) ?
  Al7 Al3 Al9 3_655 . 1_655 86.55(9) ?
  Pt1 Al4 Pt1 3_665 . 9_665 86.18(12) ?
  Pt1 Al4 Pt2 3_665 . . 116.38(8) ?
  Pt1 Al4 Pt5 3_665 . . 118.75(7) ?
  Pt1 Al4 Al1 3_665 . . 106.91(5) ?
  Pt1 Al4 Al1 3_665 . 2_665 57.58(8) ?
  Pt1 Al4 Al1 3_665 . 16_555 166.25(9) ?
  Pt1 Al4 Al1 3_665 . 17_665 101.92(11) ?
  Pt1 Al4 Al2 3_665 . . 60.81(6) ?
  Pt1 Al4 Al2 3_665 . 7_555 91.17(11) ?
  Pt1 Al4 Al2 3_665 . 16_555 132.05(17) ?
  Pt1 Al4 Al2 3_665 . 22_555 41.29(5) ?
  Pt1 Al4 Al4 3_665 . 7_555 49.90(7) ?
  Pt1 Al4 Al6 3_665 . . 81.14(4) ?
  Pt1 Al4 Al6 3_665 . 16_555 145.59(8) ?
  Pt1 Al4 Al8 3_665 . 3_665 51.68(7) ?
  Pt1 Al4 Pt2 9_665 . . 116.38(8) ?
  Pt1 Al4 Pt5 9_665 . . 118.75(7) ?
  Pt1 Al4 Al1 9_665 . . 166.25(9) ?
  Pt1 Al4 Al1 9_665 . 2_665 101.92(11) ?
  Pt1 Al4 Al1 9_665 . 16_555 106.91(5) ?
  Pt1 Al4 Al1 9_665 . 17_665 57.58(8) ?
  Pt1 Al4 Al2 9_665 . . 132.05(17) ?
  Pt1 Al4 Al2 9_665 . 7_555 41.29(5) ?
  Pt1 Al4 Al2 9_665 . 16_555 60.81(6) ?
  Pt1 Al4 Al2 9_665 . 22_555 91.17(11) ?
  Pt1 Al4 Al4 9_665 . 7_555 49.90(7) ?
  Pt1 Al4 Al6 9_665 . . 145.59(8) ?
  Pt1 Al4 Al6 9_665 . 16_555 81.14(4) ?
  Pt1 Al4 Al8 9_665 . 3_665 51.68(7) ?
  Pt2 Al4 Pt5 . . . 101.32(13) ?
  Pt2 Al4 Al1 . . . 54.33(7) ?
  Pt2 Al4 Al1 . . 2_665 141.16(10) ?
  Pt2 Al4 Al1 . . 16_555 54.33(7) ?
  Pt2 Al4 Al1 . . 17_665 141.16(10) ?
  Pt2 Al4 Al2 . . . 60.94(6) ?
  Pt2 Al4 Al2 . . 7_555 77.52(7) ?
  Pt2 Al4 Al2 . . 16_555 60.94(6) ?
  Pt2 Al4 Al2 . . 22_555 77.52(7) ?
  Pt2 Al4 Al4 . . 7_555 99.37(10) ?
  Pt2 Al4 Al6 . . . 97.87(9) ?
  Pt2 Al4 Al6 . . 16_555 97.87(9) ?
  Pt2 Al4 Al8 . . 3_665 159.37(17) ?
  Pt5 Al4 Al1 . . . 59.01(9) ?
  Pt5 Al4 Al1 . . 2_665 62.64(9) ?
  Pt5 Al4 Al1 . . 16_555 59.01(9) ?
  Pt5 Al4 Al1 . . 17_665 62.64(9) ?
  Pt5 Al4 Al2 . . . 107.84(12) ?
  Pt5 Al4 Al2 . . 7_555 145.41(5) ?
  Pt5 Al4 Al2 . . 16_555 107.84(12) ?
  Pt5 Al4 Al2 . . 22_555 145.41(5) ?
  Pt5 Al4 Al4 . . 7_555 159.31(11) ?
  Pt5 Al4 Al6 . . . 45.77(5) ?
  Pt5 Al4 Al6 . . 16_555 45.77(5) ?
  Pt5 Al4 Al8 . . 3_665 99.31(11) ?
  Al1 Al4 Al1 . . 2_665 89.00(10) ?
  Al1 Al4 Al1 . . 16_555 59.75(10) ?
  Al1 Al4 Al1 . . 17_665 121.61(15) ?
  Al1 Al4 Al2 . . . 55.46(9) ?
  Al1 Al4 Al2 . . 7_555 131.80(8) ?
  Al1 Al4 Al2 . . 16_555 106.08(12) ?
  Al1 Al4 Al2 . . 22_555 95.95(7) ?
  Al1 Al4 Al4 . . 7_555 136.74(8) ?
  Al1 Al4 Al6 . . . 44.27(5) ?
  Al1 Al4 Al6 . . 16_555 89.87(11) ?
  Al1 Al4 Al8 . . 3_665 140.51(9) ?
  Al1 Al4 Al1 2_665 . 16_555 121.61(15) ?
  Al1 Al4 Al1 2_665 . 17_665 65.86(8) ?
  Al1 Al4 Al2 2_665 . . 89.15(6) ?
  Al1 Al4 Al2 2_665 . 7_555 136.43(14) ?
  Al1 Al4 Al2 2_665 . 16_555 154.98(9) ?
  Al1 Al4 Al2 2_665 . 22_555 96.34(9) ?
  Al1 Al4 Al4 2_665 . 7_555 100.48(12) ?
  Al1 Al4 Al6 2_665 . . 44.76(7) ?
  Al1 Al4 Al6 2_665 . 16_555 93.95(10) ?
  Al1 Al4 Al8 2_665 . 3_665 51.77(9) ?
  Al1 Al4 Al1 16_555 . 17_665 89.00(10) ?
  Al1 Al4 Al2 16_555 . . 106.08(12) ?
  Al1 Al4 Al2 16_555 . 7_555 95.95(7) ?
  Al1 Al4 Al2 16_555 . 16_555 55.46(9) ?
  Al1 Al4 Al2 16_555 . 22_555 131.80(8) ?
  Al1 Al4 Al4 16_555 . 7_555 136.74(8) ?
  Al1 Al4 Al6 16_555 . . 89.87(11) ?
  Al1 Al4 Al6 16_555 . 16_555 44.27(5) ?
  Al1 Al4 Al8 16_555 . 3_665 140.51(9) ?
  Al1 Al4 Al2 17_665 . . 154.98(9) ?
  Al1 Al4 Al2 17_665 . 7_555 96.34(9) ?
  Al1 Al4 Al2 17_665 . 16_555 89.15(6) ?
  Al1 Al4 Al2 17_665 . 22_555 136.43(14) ?
  Al1 Al4 Al4 17_665 . 7_555 100.48(12) ?
  Al1 Al4 Al6 17_665 . . 93.95(10) ?
  Al1 Al4 Al6 17_665 . 16_555 44.76(7) ?
  Al1 Al4 Al8 17_665 . 3_665 51.77(9) ?
  Al2 Al4 Al2 . . 7_555 101.66(11) ?
  Al2 Al4 Al2 . . 16_555 115.82(10) ?
  Al2 Al4 Al2 . . 22_555 40.97(9) ?
  Al2 Al4 Al4 . . 7_555 82.34(11) ?
  Al2 Al4 Al6 . . . 66.84(7) ?
  Al2 Al4 Al6 . . 16_555 145.17(15) ?
  Al2 Al4 Al8 . . 3_665 112.25(10) ?
  Al2 Al4 Al2 7_555 . 16_555 40.97(9) ?
  Al2 Al4 Al2 7_555 . 22_555 68.79(8) ?
  Al2 Al4 Al4 7_555 . 7_555 41.36(6) ?
  Al2 Al4 Al6 7_555 . . 168.25(8) ?
  Al2 Al4 Al6 7_555 . 16_555 99.75(5) ?
  Al2 Al4 Al8 7_555 . 3_665 85.51(11) ?
  Al2 Al4 Al2 16_555 . 22_555 101.66(11) ?
  Al2 Al4 Al4 16_555 . 7_555 82.34(11) ?
  Al2 Al4 Al6 16_555 . . 145.17(15) ?
  Al2 Al4 Al6 16_555 . 16_555 66.84(7) ?
  Al2 Al4 Al8 16_555 . 3_665 112.25(10) ?
  Al2 Al4 Al4 22_555 . 7_555 41.36(6) ?
  Al2 Al4 Al6 22_555 . . 99.75(5) ?
  Al2 Al4 Al6 22_555 . 16_555 168.25(8) ?
  Al2 Al4 Al8 22_555 . 3_665 85.51(11) ?
  Al4 Al4 Al6 7_555 . . 130.73(6) ?
  Al4 Al4 Al6 7_555 . 16_555 130.73(6) ?
  Al4 Al4 Al8 7_555 . 3_665 60.00(11) ?
  Al6 Al4 Al6 . . 16_555 91.54(10) ?
  Al6 Al4 Al8 . . 3_665 96.48(7) ?
  Al6 Al4 Al8 16_555 . 3_665 96.48(7) ?
  Ba Al5 Ba . . 11_655 139.99(7) ?
  Ba Al5 Pt1 . . . 66.65(3) ?
  Ba Al5 Pt1 . . 11_655 92.56(3) ?
  Ba Al5 Pt3 . . 14_555 62.67(4) ?
  Ba Al5 Pt3 . . 15_655 154.87(9) ?
  Ba Al5 Al1 . . 15_655 137.51(7) ?
  Ba Al5 Al1 . . 22_555 56.80(4) ?
  Ba Al5 Al2 . . 2_655 99.71(5) ?
  Ba Al5 Al2 . . 12_555 50.81(4) ?
  Ba Al5 Al2 . . 14_555 56.74(5) ?
  Ba Al5 Al2 . . 24_655 122.65(5) ?
  Ba Al5 Al5 . . 13_655 70.00(5) ?
  Ba Al5 Al6 . . 13_665 115.19(8) ?
  Ba Al5 Al6 . . 22_555 100.92(6) ?
  Ba Al5 Pt1 11_655 . . 92.56(8) ?
  Ba Al5 Pt1 11_655 . 11_655 66.65(5) ?
  Ba Al5 Pt3 11_655 . 14_555 154.87(5) ?
  Ba Al5 Pt3 11_655 . 15_655 62.67(5) ?
  Ba Al5 Al1 11_655 . 15_655 56.80(8) ?
  Ba Al5 Al1 11_655 . 22_555 137.51(7) ?
  Ba Al5 Al2 11_655 . 2_655 50.81(5) ?
  Ba Al5 Al2 11_655 . 12_555 99.71(7) ?
  Ba Al5 Al2 11_655 . 14_555 122.65(7) ?
  Ba Al5 Al2 11_655 . 24_655 56.74(7) ?
  Ba Al5 Al5 11_655 . 13_655 70.00(8) ?
  Ba Al5 Al6 11_655 . 13_665 100.92(4) ?
  Ba Al5 Al6 11_655 . 22_555 115.19(4) ?
  Pt1 Al5 Pt1 . . 11_655 118.16(10) ?
  Pt1 Al5 Pt3 . . 14_555 110.15(6) ?
  Pt1 Al5 Pt3 . . 15_655 109.02(4) ?
  Pt1 Al5 Al1 . . 15_655 149.31(13) ?
  Pt1 Al5 Al1 . . 22_555 54.91(5) ?
  Pt1 Al5 Al2 . . 2_655 42.00(5) ?
  Pt1 Al5 Al2 . . 12_555 92.70(6) ?
  Pt1 Al5 Al2 . . 14_555 122.02(6) ?
  Pt1 Al5 Al2 . . 24_655 57.06(5) ?
  Pt1 Al5 Al5 . . 13_655 59.08(5) ?
  Pt1 Al5 Al6 . . 13_665 146.87(9) ?
  Pt1 Al5 Al6 . . 22_555 94.97(6) ?
  Pt1 Al5 Pt3 11_655 . 14_555 109.02(6) ?
  Pt1 Al5 Pt3 11_655 . 15_655 110.15(4) ?
  Pt1 Al5 Al1 11_655 . 15_655 54.91(4) ?
  Pt1 Al5 Al1 11_655 . 22_555 149.31(6) ?
  Pt1 Al5 Al2 11_655 . 2_655 92.70(9) ?
  Pt1 Al5 Al2 11_655 . 12_555 42.00(4) ?
  Pt1 Al5 Al2 11_655 . 14_555 57.06(6) ?
  Pt1 Al5 Al2 11_655 . 24_655 122.02(12) ?
  Pt1 Al5 Al5 11_655 . 13_655 59.08(5) ?
  Pt1 Al5 Al6 11_655 . 13_665 94.97(6) ?
  Pt1 Al5 Al6 11_655 . 22_555 146.87(9) ?
  Pt3 Al5 Pt3 14_555 . 15_655 98.57(9) ?
  Pt3 Al5 Al1 14_555 . 15_655 99.71(9) ?
  Pt3 Al5 Al1 14_555 . 22_555 57.97(7) ?
  Pt3 Al5 Al2 14_555 . 2_655 151.83(4) ?
  Pt3 Al5 Al2 14_555 . 12_555 90.11(7) ?
  Pt3 Al5 Al2 14_555 . 14_555 53.90(8) ?
  Pt3 Al5 Al2 14_555 . 24_655 127.32(9) ?
  Pt3 Al5 Al5 14_555 . 13_655 130.71(7) ?
  Pt3 Al5 Al6 14_555 . 13_665 54.09(6) ?
  Pt3 Al5 Al6 14_555 . 22_555 54.09(6) ?
  Pt3 Al5 Al1 15_655 . 15_655 57.97(5) ?
  Pt3 Al5 Al1 15_655 . 22_555 99.71(6) ?
  Pt3 Al5 Al2 15_655 . 2_655 90.11(7) ?
  Pt3 Al5 Al2 15_655 . 12_555 151.83(4) ?
  Pt3 Al5 Al2 15_655 . 14_555 127.32(8) ?
  Pt3 Al5 Al2 15_655 . 24_655 53.90(5) ?
  Pt3 Al5 Al5 15_655 . 13_655 130.71(12) ?
  Pt3 Al5 Al6 15_655 . 13_665 54.09(4) ?
  Pt3 Al5 Al6 15_655 . 22_555 54.09(4) ?
  Al1 Al5 Al1 15_655 . 22_555 147.80(11) ?
  Al1 Al5 Al2 15_655 . 2_655 107.55(10) ?
  Al1 Al5 Al2 15_655 . 12_555 94.25(6) ?
  Al1 Al5 Al2 15_655 . 14_555 81.32(8) ?
  Al1 Al5 Al2 15_655 . 24_655 99.10(9) ?
  Al1 Al5 Al5 15_655 . 13_655 106.10(8) ?
  Al1 Al5 Al6 15_655 . 13_665 51.82(7) ?
  Al1 Al5 Al6 15_655 . 22_555 96.87(8) ?
  Al1 Al5 Al2 22_555 . 2_655 94.25(7) ?
  Al1 Al5 Al2 22_555 . 12_555 107.55(6) ?
  Al1 Al5 Al2 22_555 . 14_555 99.10(10) ?
  Al1 Al5 Al2 22_555 . 24_655 81.32(7) ?
  Al1 Al5 Al5 22_555 . 13_655 106.10(6) ?
  Al1 Al5 Al6 22_555 . 13_665 96.87(10) ?
  Al1 Al5 Al6 22_555 . 22_555 51.82(7) ?
  Al2 Al5 Al2 2_655 . 12_555 94.75(8) ?
  Al2 Al5 Al2 2_655 . 14_555 136.62(9) ?
  Al2 Al5 Al2 2_655 . 24_655 41.87(7) ?
  Al2 Al5 Al5 2_655 . 13_655 47.38(6) ?
  Al2 Al5 Al6 2_655 . 13_665 143.79(6) ?
  Al2 Al5 Al6 2_655 . 22_555 114.26(6) ?
  Al2 Al5 Al2 12_555 . 14_555 41.87(8) ?
  Al2 Al5 Al2 12_555 . 24_655 136.62(12) ?
  Al2 Al5 Al5 12_555 . 13_655 47.38(6) ?
  Al2 Al5 Al6 12_555 . 13_665 114.26(7) ?
  Al2 Al5 Al6 12_555 . 22_555 143.79(10) ?
  Al2 Al5 Al2 14_555 . 24_655 178.49(13) ?
  Al2 Al5 Al5 14_555 . 13_655 89.25(8) ?
  Al2 Al5 Al6 14_555 . 13_665 75.09(8) ?
  Al2 Al5 Al6 14_555 . 22_555 106.31(12) ?
  Al2 Al5 Al5 24_655 . 13_655 89.25(10) ?
  Al2 Al5 Al6 24_655 . 13_665 106.31(7) ?
  Al2 Al5 Al6 24_655 . 22_555 75.09(7) ?
  Al5 Al5 Al6 13_655 . 13_665 154.05(6) ?
  Al5 Al5 Al6 13_655 . 22_555 154.05(6) ?
  Al6 Al5 Al6 13_665 . 22_555 51.90(9) ?
  Pt3 Al6 Pt3 . . 2_665 95.57(8) ?
  Pt3 Al6 Pt3 . . 3_565 95.57(8) ?
  Pt3 Al6 Pt5 . . . 121.22(6) ?
  Pt3 Al6 Al1 . . . 61.99(5) ?
  Pt3 Al6 Al1 . . 2_665 107.41(7) ?
  Pt3 Al6 Al1 . . 3_565 148.74(7) ?
  Pt3 Al6 Al2 . . . 43.00(3) ?
  Pt3 Al6 Al2 . . 2_665 136.05(7) ?
  Pt3 Al6 Al2 . . 3_565 101.48(4) ?
  Pt3 Al6 Al4 . . . 84.83(4) ?
  Pt3 Al6 Al4 . . 2_665 158.35(10) ?
  Pt3 Al6 Al4 . . 3_565 105.96(5) ?
  Pt3 Al6 Al5 . . 13_665 122.83(12) ?
  Pt3 Al6 Al5 . . 14_565 52.32(7) ?
  Pt3 Al6 Al5 . . 15_555 52.32(5) ?
  Pt3 Al6 Al6 . . 10_665 58.78(6) ?
  Pt3 Al6 Pt3 2_665 . 3_565 95.57(8) ?
  Pt3 Al6 Pt5 2_665 . . 121.22(6) ?
  Pt3 Al6 Al1 2_665 . . 148.73(6) ?
  Pt3 Al6 Al1 2_665 . 2_665 61.99(5) ?
  Pt3 Al6 Al1 2_665 . 3_565 107.41(5) ?
  Pt3 Al6 Al2 2_665 . . 101.48(4) ?
  Pt3 Al6 Al2 2_665 . 2_665 43.00(4) ?
  Pt3 Al6 Al2 2_665 . 3_565 136.05(7) ?
  Pt3 Al6 Al4 2_665 . . 105.96(6) ?
  Pt3 Al6 Al4 2_665 . 2_665 84.83(4) ?
  Pt3 Al6 Al4 2_665 . 3_565 158.35(8) ?
  Pt3 Al6 Al5 2_665 . 13_665 52.32(5) ?
  Pt3 Al6 Al5 2_665 . 14_565 122.83(12) ?
  Pt3 Al6 Al5 2_665 . 15_555 52.32(4) ?
  Pt3 Al6 Al6 2_665 . 10_665 58.78(6) ?
  Pt3 Al6 Pt5 3_565 . . 121.22(6) ?
  Pt3 Al6 Al1 3_565 . . 107.41(6) ?
  Pt3 Al6 Al1 3_565 . 2_665 148.73(6) ?
  Pt3 Al6 Al1 3_565 . 3_565 61.99(6) ?
  Pt3 Al6 Al2 3_565 . . 136.05(7) ?
  Pt3 Al6 Al2 3_565 . 2_665 101.48(6) ?
  Pt3 Al6 Al2 3_565 . 3_565 43.00(3) ?
  Pt3 Al6 Al4 3_565 . . 158.35(8) ?
  Pt3 Al6 Al4 3_565 . 2_665 105.96(8) ?
  Pt3 Al6 Al4 3_565 . 3_565 84.83(7) ?
  Pt3 Al6 Al5 3_565 . 13_665 52.32(4) ?
  Pt3 Al6 Al5 3_565 . 14_565 52.32(7) ?
  Pt3 Al6 Al5 3_565 . 15_555 122.83(12) ?
  Pt3 Al6 Al6 3_565 . 10_665 58.78(6) ?
  Pt5 Al6 Al1 . . . 63.89(8) ?
  Pt5 Al6 Al1 . . 2_665 63.89(8) ?
  Pt5 Al6 Al1 . . 3_565 63.89(8) ?
  Pt5 Al6 Al2 . . . 83.07(6) ?
  Pt5 Al6 Al2 . . 2_665 83.07(6) ?
  Pt5 Al6 Al2 . . 3_565 83.07(6) ?
  Pt5 Al6 Al4 . . . 44.23(5) ?
  Pt5 Al6 Al4 . . 2_665 44.23(5) ?
  Pt5 Al6 Al4 . . 3_565 44.23(6) ?
  Pt5 Al6 Al5 . . 13_665 115.95(6) ?
  Pt5 Al6 Al5 . . 14_565 115.95(6) ?
  Pt5 Al6 Al5 . . 15_555 115.95(6) ?
  Pt5 Al6 Al6 . . 10_665 180 ?
  Al1 Al6 Al1 . . 2_665 102.09(11) ?
  Al1 Al6 Al1 . . 3_565 102.09(11) ?
  Al1 Al6 Al2 . . . 47.27(7) ?
  Al1 Al6 Al2 . . 2_665 144.06(12) ?
  Al1 Al6 Al2 . . 3_565 73.12(7) ?
  Al1 Al6 Al4 . . . 53.85(8) ?
  Al1 Al6 Al4 . . 2_665 108.02(11) ?
  Al1 Al6 Al4 . . 3_565 48.27(8) ?
  Al1 Al6 Al5 . . 13_665 157.85(7) ?
  Al1 Al6 Al5 . . 14_565 62.21(6) ?
  Al1 Al6 Al5 . . 15_555 96.77(7) ?
  Al1 Al6 Al6 . . 10_665 116.11(8) ?
  Al1 Al6 Al1 2_665 . 3_565 102.09(12) ?
  Al1 Al6 Al2 2_665 . . 73.12(8) ?
  Al1 Al6 Al2 2_665 . 2_665 47.27(8) ?
  Al1 Al6 Al2 2_665 . 3_565 144.06(12) ?
  Al1 Al6 Al4 2_665 . . 48.27(8) ?
  Al1 Al6 Al4 2_665 . 2_665 53.85(11) ?
  Al1 Al6 Al4 2_665 . 3_565 108.02(12) ?
  Al1 Al6 Al5 2_665 . 13_665 96.77(6) ?
  Al1 Al6 Al5 2_665 . 14_565 157.85(9) ?
  Al1 Al6 Al5 2_665 . 15_555 62.21(7) ?
  Al1 Al6 Al6 2_665 . 10_665 116.11(8) ?
  Al1 Al6 Al2 3_565 . . 144.06(12) ?
  Al1 Al6 Al2 3_565 . 2_665 73.12(8) ?
  Al1 Al6 Al2 3_565 . 3_565 47.27(7) ?
  Al1 Al6 Al4 3_565 . . 108.02(12) ?
  Al1 Al6 Al4 3_565 . 2_665 48.27(10) ?
  Al1 Al6 Al4 3_565 . 3_565 53.85(8) ?
  Al1 Al6 Al5 3_565 . 13_665 62.21(6) ?
  Al1 Al6 Al5 3_565 . 14_565 96.77(9) ?
  Al1 Al6 Al5 3_565 . 15_555 157.85(7) ?
  Al1 Al6 Al6 3_565 . 10_665 116.11(8) ?
  Al2 Al6 Al2 . . 2_665 118.57(7) ?
  Al2 Al6 Al2 . . 3_565 118.57(5) ?
  Al2 Al6 Al4 . . . 42.03(5) ?
  Al2 Al6 Al4 . . 2_665 115.64(10) ?
  Al2 Al6 Al4 . . 3_565 92.92(8) ?
  Al2 Al6 Al5 . . 13_665 152.56(9) ?
  Al2 Al6 Al5 . . 14_565 84.80(7) ?
  Al2 Al6 Al5 . . 15_555 50.33(4) ?
  Al2 Al6 Al6 . . 10_665 96.93(6) ?
  Al2 Al6 Al2 2_665 . 3_565 118.57(7) ?
  Al2 Al6 Al4 2_665 . . 92.92(7) ?
  Al2 Al6 Al4 2_665 . 2_665 42.03(5) ?
  Al2 Al6 Al4 2_665 . 3_565 115.64(9) ?
  Al2 Al6 Al5 2_665 . 13_665 50.33(5) ?
  Al2 Al6 Al5 2_665 . 14_565 152.56(10) ?
  Al2 Al6 Al5 2_665 . 15_555 84.80(7) ?
  Al2 Al6 Al6 2_665 . 10_665 96.93(6) ?
  Al2 Al6 Al4 3_565 . . 115.64(9) ?
  Al2 Al6 Al4 3_565 . 2_665 92.92(8) ?
  Al2 Al6 Al4 3_565 . 3_565 42.03(7) ?
  Al2 Al6 Al5 3_565 . 13_665 84.80(5) ?
  Al2 Al6 Al5 3_565 . 14_565 50.33(7) ?
  Al2 Al6 Al5 3_565 . 15_555 152.56(9) ?
  Al2 Al6 Al6 3_565 . 10_665 96.93(6) ?
  Al4 Al6 Al4 . . 2_665 74.32(9) ?
  Al4 Al6 Al4 . . 3_565 74.32(10) ?
  Al4 Al6 Al5 . . 13_665 143.02(6) ?
  Al4 Al6 Al5 . . 14_565 114.52(7) ?
  Al4 Al6 Al5 . . 15_555 74.15(6) ?
  Al4 Al6 Al6 . . 10_665 135.77(5) ?
  Al4 Al6 Al4 2_665 . 3_565 74.32(8) ?
  Al4 Al6 Al5 2_665 . 13_665 74.15(6) ?
  Al4 Al6 Al5 2_665 . 14_565 143.02(10) ?
  Al4 Al6 Al5 2_665 . 15_555 114.52(8) ?
  Al4 Al6 Al6 2_665 . 10_665 135.77(5) ?
  Al4 Al6 Al5 3_565 . 13_665 114.52(8) ?
  Al4 Al6 Al5 3_565 . 14_565 74.15(6) ?
  Al4 Al6 Al5 3_565 . 15_555 143.02(8) ?
  Al4 Al6 Al6 3_565 . 10_665 135.77(6) ?
  Al5 Al6 Al5 13_665 . 14_565 102.28(9) ?
  Al5 Al6 Al5 13_665 . 15_555 102.28(8) ?
  Al5 Al6 Al6 13_665 . 10_665 64.05(6) ?
  Al5 Al6 Al5 14_565 . 15_555 102.28(10) ?
  Al5 Al6 Al6 14_565 . 10_665 64.05(6) ?
  Al5 Al6 Al6 15_555 . 10_665 64.05(6) ?
  Ba Al7 Ba . . 8_555 126.06(12) ?
  Ba Al7 Pt2 . . 3_555 74.17(6) ?
  Ba Al7 Pt2 . . 7_555 74.17(6) ?
  Ba Al7 Pt4 . . . 78.31(3) ?
  Ba Al7 Pt4 . . 7_555 155.63(11) ?
  Ba Al7 Al3 . . 2_545 70.90(5) ?
  Ba Al7 Al3 . . 3_665 70.90(7) ?
  Ba Al7 Al3 . . 7_545 124.45(7) ?
  Ba Al7 Al3 . . 9_665 124.45(6) ?
  Ba Al7 Al7 . . 2_555 113.13(4) ?
  Ba Al7 Al7 . . 3_555 113.13(5) ?
  Ba Al7 Al8 . . . 63.03(6) ?
  Ba Al7 Pt2 8_555 . 3_555 74.17(6) ?
  Ba Al7 Pt2 8_555 . 7_555 74.17(6) ?
  Ba Al7 Pt4 8_555 . . 155.63(11) ?
  Ba Al7 Pt4 8_555 . 7_555 78.31(3) ?
  Ba Al7 Al3 8_555 . 2_545 124.45(7) ?
  Ba Al7 Al3 8_555 . 3_665 124.45(6) ?
  Ba Al7 Al3 8_555 . 7_545 70.90(5) ?
  Ba Al7 Al3 8_555 . 9_665 70.90(7) ?
  Ba Al7 Al7 8_555 . 2_555 113.13(4) ?
  Ba Al7 Al7 8_555 . 3_555 113.13(5) ?
  Ba Al7 Al8 8_555 . . 63.03(6) ?
  Pt2 Al7 Pt2 3_555 . 7_555 106.07(13) ?
  Pt2 Al7 Pt4 3_555 . . 118.01(3) ?
  Pt2 Al7 Pt4 3_555 . 7_555 118.01(3) ?
  Pt2 Al7 Al3 3_555 . 2_545 59.95(5) ?
  Pt2 Al7 Al3 3_555 . 3_665 144.78(11) ?
  Pt2 Al7 Al3 3_555 . 7_545 59.95(5) ?
  Pt2 Al7 Al3 3_555 . 9_665 144.78(11) ?
  Pt2 Al7 Al7 3_555 . 2_555 156.97(10) ?
  Pt2 Al7 Al7 3_555 . 3_555 96.97(8) ?
  Pt2 Al7 Al8 3_555 . . 53.03(7) ?
  Pt2 Al7 Pt4 7_555 . . 118.01(3) ?
  Pt2 Al7 Pt4 7_555 . 7_555 118.01(3) ?
  Pt2 Al7 Al3 7_555 . 2_545 144.78(10) ?
  Pt2 Al7 Al3 7_555 . 3_665 59.95(6) ?
  Pt2 Al7 Al3 7_555 . 7_545 144.78(10) ?
  Pt2 Al7 Al3 7_555 . 9_665 59.95(6) ?
  Pt2 Al7 Al7 7_555 . 2_555 96.97(5) ?
  Pt2 Al7 Al7 7_555 . 3_555 156.97(12) ?
  Pt2 Al7 Al8 7_555 . . 53.03(7) ?
  Pt4 Al7 Pt4 . . 7_555 77.32(11) ?
  Pt4 Al7 Al3 . . 2_545 58.78(7) ?
  Pt4 Al7 Al3 . . 3_665 58.78(7) ?
  Pt4 Al7 Al3 . . 7_545 96.18(10) ?
  Pt4 Al7 Al3 . . 9_665 96.18(11) ?
  Pt4 Al7 Al7 . . 2_555 47.45(6) ?
  Pt4 Al7 Al7 . . 3_555 47.45(7) ?
  Pt4 Al7 Al8 . . . 141.34(6) ?
  Pt4 Al7 Al3 7_555 . 2_545 96.18(10) ?
  Pt4 Al7 Al3 7_555 . 3_665 96.18(11) ?
  Pt4 Al7 Al3 7_555 . 7_545 58.78(7) ?
  Pt4 Al7 Al3 7_555 . 9_665 58.78(7) ?
  Pt4 Al7 Al7 7_555 . 2_555 47.45(6) ?
  Pt4 Al7 Al7 7_555 . 3_555 47.45(7) ?
  Pt4 Al7 Al8 7_555 . . 141.34(6) ?
  Al3 Al7 Al3 2_545 . 3_665 111.09(10) ?
  Al3 Al7 Al3 2_545 . 7_545 60.12(9) ?
  Al3 Al7 Al3 2_545 . 9_665 149.51(17) ?
  Al3 Al7 Al7 2_545 . 2_555 100.64(11) ?
  Al3 Al7 Al7 2_545 . 3_555 50.21(8) ?
  Al3 Al7 Al8 2_545 . . 105.25(9) ?
  Al3 Al7 Al3 3_665 . 7_545 149.51(17) ?
  Al3 Al7 Al3 3_665 . 9_665 60.12(9) ?
  Al3 Al7 Al7 3_665 . 2_555 50.21(8) ?
  Al3 Al7 Al7 3_665 . 3_555 100.64(13) ?
  Al3 Al7 Al8 3_665 . . 105.25(10) ?
  Al3 Al7 Al3 7_545 . 9_665 111.09(10) ?
  Al3 Al7 Al7 7_545 . 2_555 100.64(11) ?
  Al3 Al7 Al7 7_545 . 3_555 50.21(8) ?
  Al3 Al7 Al8 7_545 . . 105.25(9) ?
  Al3 Al7 Al7 9_665 . 2_555 50.21(8) ?
  Al3 Al7 Al7 9_665 . 3_555 100.64(13) ?
  Al3 Al7 Al8 9_665 . . 105.25(10) ?
  Al7 Al7 Al7 2_555 . 3_555 60.00(10) ?
  Al7 Al7 Al8 2_555 . . 150.00(4) ?
  Al7 Al7 Al8 3_555 . . 150.00(7) ?
  Ba Al8 Ba . . 8_555 123.43(12) ?
  Ba Al8 Pt1 . . . 76.774(13) ?
  Ba Al8 Pt1 . . 8_555 159.80(12) ?
  Ba Al8 Pt2 . . 3_555 73.60(6) ?
  Ba Al8 Pt2 . . 7_555 73.60(6) ?
  Ba Al8 Al1 . . 3_555 67.14(7) ?
  Ba Al8 Al1 . . 7_555 126.58(7) ?
  Ba Al8 Al1 . . 18_555 126.58(6) ?
  Ba Al8 Al1 . . 22_555 67.14(5) ?
  Ba Al8 Al4 . . 2_655 114.23(4) ?
  Ba Al8 Al4 . . 9_655 114.23(5) ?
  Ba Al8 Al7 . . . 61.71(6) ?
  Ba Al8 Pt1 8_555 . . 159.80(12) ?
  Ba Al8 Pt1 8_555 . 8_555 76.774(13) ?
  Ba Al8 Pt2 8_555 . 3_555 73.60(6) ?
  Ba Al8 Pt2 8_555 . 7_555 73.60(6) ?
  Ba Al8 Al1 8_555 . 3_555 126.58(6) ?
  Ba Al8 Al1 8_555 . 7_555 67.14(5) ?
  Ba Al8 Al1 8_555 . 18_555 67.14(7) ?
  Ba Al8 Al1 8_555 . 22_555 126.58(7) ?
  Ba Al8 Al4 8_555 . 2_655 114.23(4) ?
  Ba Al8 Al4 8_555 . 9_655 114.23(5) ?
  Ba Al8 Al7 8_555 . . 61.71(6) ?
  Pt1 Al8 Pt1 . . 8_555 83.02(12) ?
  Pt1 Al8 Pt2 . . 3_555 116.49(3) ?
  Pt1 Al8 Pt2 . . 7_555 116.49(2) ?
  Pt1 Al8 Al1 . . 3_555 57.70(7) ?
  Pt1 Al8 Al1 . . 7_555 101.92(11) ?
  Pt1 Al8 Al1 . . 18_555 101.92(12) ?
  Pt1 Al8 Al1 . . 22_555 57.70(7) ?
  Pt1 Al8 Al4 . . 2_655 49.57(7) ?
  Pt1 Al8 Al4 . . 9_655 49.57(7) ?
  Pt1 Al8 Al7 . . . 138.49(6) ?
  Pt1 Al8 Pt2 8_555 . 3_555 116.49(3) ?
  Pt1 Al8 Pt2 8_555 . 7_555 116.49(2) ?
  Pt1 Al8 Al1 8_555 . 3_555 101.92(12) ?
  Pt1 Al8 Al1 8_555 . 7_555 57.70(7) ?
  Pt1 Al8 Al1 8_555 . 18_555 57.70(7) ?
  Pt1 Al8 Al1 8_555 . 22_555 101.92(11) ?
  Pt1 Al8 Al4 8_555 . 2_655 49.57(7) ?
  Pt1 Al8 Al4 8_555 . 9_655 49.57(7) ?
  Pt1 Al8 Al7 8_555 . . 138.49(6) ?
  Pt2 Al8 Pt2 3_555 . 7_555 106.88(15) ?
  Pt2 Al8 Al1 3_555 . 3_555 59.20(6) ?
  Pt2 Al8 Al1 3_555 . 7_555 140.60(10) ?
  Pt2 Al8 Al1 3_555 . 18_555 59.20(6) ?
  Pt2 Al8 Al1 3_555 . 22_555 140.60(10) ?
  Pt2 Al8 Al4 3_555 . 2_655 96.56(6) ?
  Pt2 Al8 Al4 3_555 . 9_655 156.55(14) ?
  Pt2 Al8 Al7 3_555 . . 53.44(7) ?
  Pt2 Al8 Al1 7_555 . 3_555 140.60(11) ?
  Pt2 Al8 Al1 7_555 . 7_555 59.20(6) ?
  Pt2 Al8 Al1 7_555 . 18_555 140.60(11) ?
  Pt2 Al8 Al1 7_555 . 22_555 59.20(6) ?
  Pt2 Al8 Al4 7_555 . 2_655 156.55(12) ?
  Pt2 Al8 Al4 7_555 . 9_655 96.56(9) ?
  Pt2 Al8 Al7 7_555 . . 53.44(7) ?
  Al1 Al8 Al1 3_555 . 7_555 154.71(19) ?
  Al1 Al8 Al1 3_555 . 18_555 67.97(7) ?
  Al1 Al8 Al1 3_555 . 22_555 106.21(8) ?
  Al1 Al8 Al4 3_555 . 2_655 53.88(10) ?
  Al1 Al8 Al4 3_555 . 9_655 102.14(15) ?
  Al1 Al8 Al7 3_555 . . 102.64(11) ?
  Al1 Al8 Al1 7_555 . 18_555 106.21(8) ?
  Al1 Al8 Al1 7_555 . 22_555 67.97(7) ?
  Al1 Al8 Al4 7_555 . 2_655 102.14(13) ?
  Al1 Al8 Al4 7_555 . 9_655 53.88(10) ?
  Al1 Al8 Al7 7_555 . . 102.64(10) ?
  Al1 Al8 Al1 18_555 . 22_555 154.71(19) ?
  Al1 Al8 Al4 18_555 . 2_655 53.88(10) ?
  Al1 Al8 Al4 18_555 . 9_655 102.14(15) ?
  Al1 Al8 Al7 18_555 . . 102.64(11) ?
  Al1 Al8 Al4 22_555 . 2_655 102.14(13) ?
  Al1 Al8 Al4 22_555 . 9_655 53.88(10) ?
  Al1 Al8 Al7 22_555 . . 102.64(10) ?
  Al4 Al8 Al4 2_655 . 9_655 59.99(12) ?
  Al4 Al8 Al7 2_655 . . 150.00(6) ?
  Al4 Al8 Al7 9_655 . . 150.00(9) ?
  Ba Al9 Ba . . 2_555 112.120(7) ?
  Ba Al9 Ba . . 3_555 112.120(13) ?
  Ba Al9 Ba . . 10_555 67.880(7) ?
  Ba Al9 Ba . . 11_555 180 ?
  Ba Al9 Ba . . 12_555 67.880(13) ?
  Ba Al9 Pt4 . . . 73.329(8) ?
  Ba Al9 Pt4 . . 10_555 106.671(8) ?
  Ba Al9 Al3 . . 1_455 118.51(5) ?
  Ba Al9 Al3 . . 2_545 57.181(10) ?
  Ba Al9 Al3 . . 3_665 57.18(5) ?
  Ba Al9 Al3 . . 10_565 122.819(10) ?
  Ba Al9 Al3 . . 11_655 61.49(5) ?
  Ba Al9 Al3 . . 12_445 122.82(5) ?
  Ba Al9 Ba 2_555 . 3_555 112.120(13) ?
  Ba Al9 Ba 2_555 . 10_555 180 ?
  Ba Al9 Ba 2_555 . 11_555 67.880(7) ?
  Ba Al9 Ba 2_555 . 12_555 67.880(13) ?
  Ba Al9 Pt4 2_555 . . 73.329(8) ?
  Ba Al9 Pt4 2_555 . 10_555 106.671(8) ?
  Ba Al9 Al3 2_555 . 1_455 57.181(10) ?
  Ba Al9 Al3 2_555 . 2_545 118.51(5) ?
  Ba Al9 Al3 2_555 . 3_665 57.18(5) ?
  Ba Al9 Al3 2_555 . 10_565 61.49(5) ?
  Ba Al9 Al3 2_555 . 11_655 122.819(10) ?
  Ba Al9 Al3 2_555 . 12_445 122.82(5) ?
  Ba Al9 Ba 3_555 . 10_555 67.880(13) ?
  Ba Al9 Ba 3_555 . 11_555 67.880(13) ?
  Ba Al9 Ba 3_555 . 12_555 180 ?
  Ba Al9 Pt4 3_555 . . 73.329(8) ?
  Ba Al9 Pt4 3_555 . 10_555 106.671(8) ?
  Ba Al9 Al3 3_555 . 1_455 57.181(13) ?
  Ba Al9 Al3 3_555 . 2_545 57.181(13) ?
  Ba Al9 Al3 3_555 . 3_665 118.51(4) ?
  Ba Al9 Al3 3_555 . 10_565 122.819(13) ?
  Ba Al9 Al3 3_555 . 11_655 122.819(13) ?
  Ba Al9 Al3 3_555 . 12_445 61.49(4) ?
  Ba Al9 Ba 10_555 . 11_555 112.120(7) ?
  Ba Al9 Ba 10_555 . 12_555 112.120(13) ?
  Ba Al9 Pt4 10_555 . . 106.671(8) ?
  Ba Al9 Pt4 10_555 . 10_555 73.329(8) ?
  Ba Al9 Al3 10_555 . 1_455 122.819(10) ?
  Ba Al9 Al3 10_555 . 2_545 61.49(5) ?
  Ba Al9 Al3 10_555 . 3_665 122.82(5) ?
  Ba Al9 Al3 10_555 . 10_565 118.51(5) ?
  Ba Al9 Al3 10_555 . 11_655 57.181(10) ?
  Ba Al9 Al3 10_555 . 12_445 57.18(5) ?
  Ba Al9 Ba 11_555 . 12_555 112.120(13) ?
  Ba Al9 Pt4 11_555 . . 106.671(8) ?
  Ba Al9 Pt4 11_555 . 10_555 73.329(8) ?
  Ba Al9 Al3 11_555 . 1_455 61.49(5) ?
  Ba Al9 Al3 11_555 . 2_545 122.819(10) ?
  Ba Al9 Al3 11_555 . 3_665 122.82(5) ?
  Ba Al9 Al3 11_555 . 10_565 57.181(10) ?
  Ba Al9 Al3 11_555 . 11_655 118.51(5) ?
  Ba Al9 Al3 11_555 . 12_445 57.18(5) ?
  Ba Al9 Pt4 12_555 . . 106.671(8) ?
  Ba Al9 Pt4 12_555 . 10_555 73.329(8) ?
  Ba Al9 Al3 12_555 . 1_455 122.819(13) ?
  Ba Al9 Al3 12_555 . 2_545 122.819(13) ?
  Ba Al9 Al3 12_555 . 3_665 61.49(4) ?
  Ba Al9 Al3 12_555 . 10_565 57.181(13) ?
  Ba Al9 Al3 12_555 . 11_655 57.181(13) ?
  Ba Al9 Al3 12_555 . 12_445 118.51(4) ?
  Pt4 Al9 Pt4 . . 10_555 180 ?
  Pt4 Al9 Al3 . . 1_455 45.18(5) ?
  Pt4 Al9 Al3 . . 2_545 45.18(5) ?
  Pt4 Al9 Al3 . . 3_665 45.18(4) ?
  Pt4 Al9 Al3 . . 10_565 134.82(5) ?
  Pt4 Al9 Al3 . . 11_655 134.82(5) ?
  Pt4 Al9 Al3 . . 12_445 134.82(4) ?
  Pt4 Al9 Al3 10_555 . 1_455 134.82(5) ?
  Pt4 Al9 Al3 10_555 . 2_545 134.82(5) ?
  Pt4 Al9 Al3 10_555 . 3_665 134.82(4) ?
  Pt4 Al9 Al3 10_555 . 10_565 45.18(5) ?
  Pt4 Al9 Al3 10_555 . 11_655 45.18(5) ?
  Pt4 Al9 Al3 10_555 . 12_445 45.18(4) ?
  Al3 Al9 Al3 1_455 . 2_545 75.81(5) ?
  Al3 Al9 Al3 1_455 . 3_665 75.81(6) ?
  Al3 Al9 Al3 1_455 . 10_565 104.19(5) ?
  Al3 Al9 Al3 1_455 . 11_655 180 ?
  Al3 Al9 Al3 1_455 . 12_445 104.19(6) ?
  Al3 Al9 Al3 2_545 . 3_665 75.81(6) ?
  Al3 Al9 Al3 2_545 . 10_565 180 ?
  Al3 Al9 Al3 2_545 . 11_655 104.19(5) ?
  Al3 Al9 Al3 2_545 . 12_445 104.19(6) ?
  Al3 Al9 Al3 3_665 . 10_565 104.19(6) ?
  Al3 Al9 Al3 3_665 . 11_655 104.19(6) ?
  Al3 Al9 Al3 3_665 . 12_445 180 ?
  Al3 Al9 Al3 10_565 . 11_655 75.81(5) ?
  Al3 Al9 Al3 10_565 . 12_445 75.81(6) ?
  Al3 Al9 Al3 11_655 . 12_445 75.81(6) ?

loop_
 _geom_torsion_atom_site_label_1
 _geom_torsion_atom_site_label_2
 _geom_torsion_atom_site_label_3
 _geom_torsion_atom_site_label_4
 _geom_torsion_site_symmetry_1
 _geom_torsion_site_symmetry_2
 _geom_torsion_site_symmetry_3
 _geom_torsion_site_symmetry_4
 _geom_torsion
 _geom_torsion_publ_flag
 ? ? ? ? ? ? ? ? ? ?

loop_
 _geom_hbond_atom_site_label_D
 _geom_hbond_atom_site_label_H
 _geom_hbond_atom_site_label_A
 _geom_hbond_site_symmetry_D
 _geom_hbond_site_symmetry_H
 _geom_hbond_site_symmetry_A
 _geom_hbond_distance_DH
 _geom_hbond_distance_HA
 _geom_hbond_distance_DA
 _geom_hbond_angle_DHA
 _geom_hbond_publ_flag
 ? ? ? ? ? ? ? ? ? ? ?


#=======================================================================

# 11. STRUCTURE-FACTOR LIST



